#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:21:53 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179478 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/75/4337517.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4337517
loop_
_publ_author_name
'Holland, Michael'
'Donakowski, Martin D.'
'Pozzi, Eric A.'
'Rasmussen, Andrew M.'
'Tran, Thanh Thao'
'Pease-Dodson, Shannon E'
'Halasyamani, P. Shiv'
'Seideman, Tamar'
'Van Duyne, Richard P.'
'Poeppelmeier, Kenneth R.'
_publ_section_title
;
 Polar alignment of Λ-shaped basic building units within transition metal
 oxide fluoride materials.
;
_journal_issue                   1
_journal_name_full               'Inorganic chemistry'
_journal_page_first              221
_journal_page_last               228
_journal_paper_doi               10.1021/ic402177j
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety         '2(F27 O6 V6), F27 O6 V6, Cl, 2(F), 30(K)'
_chemical_formula_sum            'Cl F83 K30 O18 V18'
_chemical_formula_weight         3990.37
_chemical_name_systematic
;
 ? 
;
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2012-11-06
_audit_creation_method
;
  Olex2 1.2
  (compiled Oct 26 2012 17:09:49, GUI svn.r4371)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   19.2623(6)
_cell_length_b                   19.2623(6)
_cell_length_c                   7.7318(2)
_cell_measurement_reflns_used    9997
_cell_measurement_temperature    100
_cell_measurement_theta_max      30.090
_cell_measurement_theta_min      2.904
_cell_volume                     2484.43(13)
_computing_cell_refinement       'SAINT V7.23A (Bruker, 2005)'
_computing_data_collection       'APEX2 V2.1-4 (Bruker, 2007)'
_computing_data_reduction        'SAINT v7.68A (Bruker, 2009)'
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
XL, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_computing_structure_solution
;
XS, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_diffrn_ambient_temperature      100.07
_diffrn_detector_area_resol_mean 8
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0760
_diffrn_reflns_av_unetI/netI     0.0279
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            24701
_diffrn_reflns_theta_full        30.12
_diffrn_reflns_theta_max         30.12
_diffrn_reflns_theta_min         1.22
_diffrn_source                   'sealed tube'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.085
_exptl_absorpt_correction_T_max  0.7085
_exptl_absorpt_correction_T_min  0.3330
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'Face-Indexed (Sheldrick)'
_exptl_crystal_colour            'clear yellow'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    yellow
_exptl_crystal_density_diffrn    2.667
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1892
_exptl_crystal_size_max          0.457
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.12
_refine_diff_density_max         2.669
_refine_diff_density_min         -1.301
_refine_diff_density_rms         0.266
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.132
_refine_ls_matrix_type           full
_refine_ls_number_parameters     139
_refine_ls_number_reflns         2642
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.132
_refine_ls_R_factor_all          0.0623
_refine_ls_R_factor_gt           0.0613
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0966P)²+19.6518P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1754
_refine_ls_wR_factor_ref         0.1774
_reflns_number_gt                2596
_reflns_number_total             2642
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic402177j_si_001.cif
_cod_data_source_block           Compound_1
_cod_database_code               4337517
#BEGIN Tags that were not found in dictionaries:
_olex2_refinement_description
;
1. Others
 Sof(F1D)=1-Sof(F2D)
;
#END Tags that were not found in dictionaries
loop_
_space_group_symop_id
_symmetry_equiv_pos_as_xyz
1 'x, y, z'
2 '-y, x-y, z'
3 '-x+y, -x, z'
4 'x-y, -y, -z'
5 '-x, -x+y, -z'
6 'y, x, -z'
7 '-x, -y, -z'
8 'y, -x+y, -z'
9 'x-y, x, -z'
10 '-x+y, y, z'
11 'x, x-y, z'
12 '-y, -x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
V1 V 0.13723(5) 0.27447(11) 0.74472(19) 0.0152(3) Uani 1 2 d S
V2 V 0.20403(5) 0.40806(11) 1.2045(2) 0.0160(3) Uani 1 2 d S
V3 V 0.46272(4) 0.53728(4) 0.71492(19) 0.0095(3) Uani 1 2 d S
K1 K 0.19370(15) 0.09685(7) 0.8124(3) 0.0242(4) Uani 1 2 d S
K2 K 0.32334(10) 0.32334(10) 1.0000 0.0156(3) Uani 1 2 d S
K3 K 0.34679(10) 0.34679(10) 0.5000 0.0126(3) Uani 1 2 d S
K4 K 0.42752(6) 0.57248(6) 1.2608(3) 0.0177(4) Uani 1 2 d S
K5 K 0.24878(9) 0.49755(17) 0.7669(3) 0.0252(5) Uani 1 2 d S
Cl1 Cl 0.0000 0.0000 0.5000 0.0186(9) Uani 1 12 d S
F1 F 0.1743(3) 0.2165(3) 0.8507(7) 0.0317(10) Uani 1 1 d .
F1D F 0.3333 0.6667 0.589(10) 0.08(2) Uani 0.40(5) 6 d SP
F2 F 0.2422(3) 0.3521(3) 0.7054(7) 0.0325(11) Uani 1 1 d .
F2D F 0.3333 0.6667 0.943(11) 0.16(4) Uani 0.60(5) 6 d SP
F3 F 0.16564(18) 0.3313(4) 0.9920(7) 0.0205(11) Uani 1 2 d S
F4 F 0.2367(2) 0.3379(3) 0.2771(5) 0.0196(8) Uani 1 1 d .
F5 F 0.1638(3) 0.4609(3) 1.0791(6) 0.0242(9) Uani 1 1 d .
F6 F 0.5000 0.5000 0.5000 0.0189(14) Uani 1 4 d S
F7 F 0.4310(2) 0.4354(2) 0.7860(5) 0.0150(7) Uani 1 1 d .
F8 F 0.1290(2) 0.4989(2) 0.5875(5) 0.0172(7) Uani 1 1 d .
O1 O 0.1161(3) 0.2322(6) 0.5628(11) 0.038(2) Uani 1 2 d S
O2 O 0.2327(3) 0.4654(6) 1.3639(11) 0.036(2) Uani 1 2 d S
O3 O 0.4339(2) 0.5661(2) 0.8785(8) 0.0182(13) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
K1 V1 K2 65.96(3) 9_557 .
K1 V1 K2 65.96(3) 9_557 9_557
K1 V1 K3 123.187(18) 9_557 .
K1 V1 K3 123.184(18) 9_557 9_556
K1 V1 K5 108.84(6) 9_557 .
K2 V1 K2 111.12(4) 9_557 .
K2 V1 K3 59.768(19) . .
K2 V1 K3 149.95(6) . 9_556
K2 V1 K3 59.768(19) 9_557 9_556
K2 V1 K3 149.95(6) 9_557 .
K3 V1 K3 112.21(4) 9_556 .
K5 V1 K2 76.13(4) . 9_557
K5 V1 K2 76.13(4) . .
K5 V1 K3 73.86(4) . .
K5 V1 K3 73.87(4) . 9_556
F1 V1 K1 51.58(17) . 9_557
F1 V1 K1 51.57(17) 10 9_557
F1 V1 K2 45.05(16) 10 9_557
F1 V1 K2 117.54(18) 10 .
F1 V1 K2 117.54(18) . 9_557
F1 V1 K2 45.05(16) . .
F1 V1 K3 77.74(17) 10 9_556
F1 V1 K3 77.74(17) . .
F1 V1 K3 164.59(17) 10 .
F1 V1 K3 164.59(17) . 9_556
F1 V1 K5 121.12(17) 10 .
F1 V1 K5 121.12(17) . .
F1 V1 F1 90.2(3) 10 .
F1 V1 F2 160.7(3) . 10
F1 V1 F2 87.9(2) 10 10
F1 V1 F2 87.9(2) . .
F1 V1 F2 160.7(3) 10 .
F1 V1 F3 80.2(2) 10 .
F1 V1 F3 80.2(2) . .
F2 V1 K1 114.25(17) . 9_557
F2 V1 K1 114.25(17) 10 9_557
F2 V1 K2 120.34(18) 10 .
F2 V1 K2 120.34(18) . 9_557
F2 V1 K2 50.48(17) 10 9_557
F2 V1 K2 50.48(17) . .
F2 V1 K3 30.38(17) 10 9_556
F2 V1 K3 106.63(18) . 9_556
F2 V1 K3 30.38(17) . .
F2 V1 K3 106.63(18) 10 .
F2 V1 K5 46.02(17) 10 .
F2 V1 K5 46.02(17) . .
F2 V1 F2 87.6(4) 10 .
F2 V1 F3 80.5(2) . .
F2 V1 F3 80.5(2) 10 .
F3 V1 K1 47.84(16) . 9_557
F3 V1 K2 55.65(14) . 9_557
F3 V1 K2 55.65(14) . .
F3 V1 K3 106.75(9) . .
F3 V1 K3 106.75(9) . 9_556
F3 V1 K5 61.00(16) . .
O1 V1 K1 131.9(4) . 9_557
O1 V1 K2 124.3(3) . 9_557
O1 V1 K2 124.3(3) . .
O1 V1 K3 73.39(17) . 9_556
O1 V1 K3 73.39(17) . .
O1 V1 K5 119.3(4) . .
O1 V1 F1 99.6(3) . .
O1 V1 F1 99.6(3) . 10
O1 V1 F2 99.7(3) . 10
O1 V1 F2 99.7(3) . .
O1 V1 F3 179.7(4) . .
K1 V2 K2 67.04(4) 9_557 9_557
K1 V2 K2 67.04(4) 9_557 .
K1 V2 K4 135.15(4) 9_557 3_565
K1 V2 K4 135.15(4) 9_557 .
K1 V2 K5 111.72(7) 9_557 .
K2 V2 K2 111.49(6) 9_557 .
K2 V2 K4 74.52(4) . .
K2 V2 K4 152.89(6) 9_557 .
K2 V2 K4 74.52(4) 9_557 3_565
K2 V2 K4 152.89(6) . 3_565
K4 V2 K4 88.84(7) . 3_565
K5 V2 K2 76.55(3) . 9_557
K5 V2 K2 76.55(3) . .
K5 V2 K4 79.50(5) . .
K5 V2 K4 79.50(5) . 3_565
F3 V2 K1 49.97(16) . 9_557
F3 V2 K2 55.84(3) . 9_557
F3 V2 K2 55.83(15) . .
F3 V2 K4 121.47(10) . .
F3 V2 K4 121.47(10) . 3_565
F3 V2 K5 61.75(17) . .
F4 V2 K1 51.36(14) 1_556 9_557
F4 V2 K1 51.36(14) 10_556 9_557
F4 V2 K2 45.86(12) 1_556 .
F4 V2 K2 118.38(16) 10_556 .
F4 V2 K2 45.86(12) 10_556 9_557
F4 V2 K2 118.38(16) 1_556 9_557
F4 V2 K4 85.31(14) 1_556 .
F4 V2 K4 155.59(14) 10_556 .
F4 V2 K4 85.31(14) 10_556 3_565
F4 V2 K4 155.59(14) 1_556 3_565
F4 V2 K5 122.40(13) 10_556 .
F4 V2 K5 122.40(13) 1_556 .
F4 V2 F3 81.35(18) 1_556 .
F4 V2 F3 81.35(18) 10_556 .
F4 V2 F4 90.3(3) 10_556 1_556
F5 V2 K1 117.44(16) . 9_557
F5 V2 K1 117.44(16) 10 9_557
F5 V2 K2 51.68(15) . 9_557
F5 V2 K2 122.46(15) 10 9_557
F5 V2 K2 122.46(15) . .
F5 V2 K2 51.67(15) 10 .
F5 V2 K4 102.13(16) . .
F5 V2 K4 39.70(15) 10 .
F5 V2 K4 102.13(16) 10 3_565
F5 V2 K4 39.70(15) . 3_565
F5 V2 K5 47.34(14) 10 .
F5 V2 K5 47.34(14) . .
F5 V2 F3 83.01(19) 10 .
F5 V2 F3 83.01(19) . .
F5 V2 F4 164.3(2) 10 10_556
F5 V2 F4 88.32(19) 10 1_556
F5 V2 F4 164.3(2) . 1_556
F5 V2 F4 88.32(19) . 10_556
F5 V2 F5 88.8(3) . 10
O2 V2 K1 129.9(4) . 9_557
O2 V2 K2 124.2(3) . 9_557
O2 V2 K2 124.2(3) . .
O2 V2 K4 58.6(2) . 3_565
O2 V2 K4 58.6(2) . .
O2 V2 K5 118.4(4) . .
O2 V2 F3 179.9(4) . .
O2 V2 F4 98.6(3) . 1_556
O2 V2 F4 98.6(3) . 10_556
O2 V2 F5 97.1(3) . .
O2 V2 F5 97.1(3) . 10
K3 V3 K3 109.76(5) . 7_666
K3 V3 K4 70.89(3) . 1_554
K3 V3 K4 70.89(3) 7_666 1_554
K3 V3 K4 71.29(3) . 7_667
K3 V3 K4 71.29(3) 7_666 7_667
K3 V3 K5 77.73(4) . .
K3 V3 K5 146.54(6) 7_666 .
K3 V3 K5 77.73(4) 7_666 2_665
K3 V3 K5 146.54(6) . 2_665
K4 V3 K4 111.42(5) 7_667 1_554
K4 V3 K5 139.01(5) 7_667 2_665
K4 V3 K5 81.85(5) 1_554 2_665
K4 V3 K5 139.01(5) 7_667 .
K4 V3 K5 81.85(5) 1_554 .
K5 V3 K5 79.57(9) . 2_665
F6 V3 K3 54.88(3) . .
F6 V3 K3 54.88(3) . 7_666
F6 V3 K4 55.31(5) . 1_554
F6 V3 K4 56.12(4) . 7_667
F6 V3 K5 122.71(5) . .
F6 V3 K5 122.71(5) . 2_665
F7 V3 K3 119.64(14) . 7_666
F7 V3 K3 119.64(14) 12_665 .
F7 V3 K3 48.73(11) 12_665 7_666
F7 V3 K3 48.73(11) . .
F7 V3 K4 48.99(13) 12_665 7_667
F7 V3 K4 48.99(13) . 7_667
F7 V3 K4 119.28(12) . 1_554
F7 V3 K4 119.27(12) 12_665 1_554
F7 V3 K5 155.26(14) . 2_665
F7 V3 K5 90.30(14) . .
F7 V3 K5 90.30(13) 12_665 2_665
F7 V3 K5 155.26(14) 12_665 .
F7 V3 F6 81.75(13) 12_665 .
F7 V3 F6 81.75(13) . .
F7 V3 F7 89.7(2) 12_665 .
F7 V3 F8 164.02(19) . 2_665
F7 V3 F8 164.02(19) 12_665 10
F7 V3 F8 89.62(17) . 10
F7 V3 F8 89.62(17) 12_665 2_665
F8 V3 K3 50.38(13) 2_665 7_666
F8 V3 K3 50.38(13) 10 .
F8 V3 K3 118.99(13) 2_665 .
F8 V3 K3 118.99(13) 10 7_666
F8 V3 K4 48.41(12) 10 1_554
F8 V3 K4 48.41(12) 2_665 1_554
F8 V3 K4 121.30(13) 2_665 7_667
F8 V3 K4 121.30(13) 10 7_667
F8 V3 K5 96.90(14) 10 2_665
F8 V3 K5 40.72(13) 2_665 2_665
F8 V3 K5 40.72(13) 10 .
F8 V3 K5 96.90(14) 2_665 .
F8 V3 F6 82.35(13) 10 .
F8 V3 F6 82.35(13) 2_665 .
F8 V3 F8 86.6(3) 10 2_665
O3 V3 K3 125.12(14) . 7_666
O3 V3 K3 125.12(14) . .
O3 V3 K4 124.3(3) . 7_667
O3 V3 K4 124.3(3) . 1_554
O3 V3 K5 57.03(17) . 2_665
O3 V3 K5 57.03(18) . .
O3 V3 F6 179.6(3) . .
O3 V3 F7 98.5(2) . .
O3 V3 F7 98.5(2) . 12_665
O3 V3 F8 97.4(2) . 2_665
O3 V3 F8 97.4(2) . 10
V1 K1 K2 58.16(3) 8_557 8_557
V1 K1 K2 58.16(3) 8_557 .
V2 K1 V1 70.61(5) 8_557 8_557
V2 K1 K2 58.71(4) 8_557 8_557
V2 K1 K2 58.71(4) 8_557 .
K2 K1 K2 100.19(5) . 8_557
F1 K1 V1 86.43(13) 11 8_557
F1 K1 V1 86.43(13) . 8_557
F1 K1 V1 28.78(9) 8_557 8_557
F1 K1 V1 28.78(9) 6_557 8_557
F1 K1 V2 97.58(12) . 8_557
F1 K1 V2 97.58(12) 11 8_557
F1 K1 V2 84.42(11) 6_557 8_557
F1 K1 V2 84.42(11) 8_557 8_557
F1 K1 K2 141.41(14) . 8_557
F1 K1 K2 86.93(10) 8_557 .
F1 K1 K2 43.82(10) 6_557 .
F1 K1 K2 43.17(12) . .
F1 K1 K2 141.41(14) 11 .
F1 K1 K2 43.17(11) 11 8_557
F1 K1 K2 43.82(10) 8_557 8_557
F1 K1 K2 86.93(10) 6_557 8_557
F1 K1 F1 109.94(13) 11 6_557
F1 K1 F1 58.89(19) . 6_557
F1 K1 F1 160.0(3) 11 .
F1 K1 F1 58.89(19) 11 8_557
F1 K1 F1 109.94(13) . 8_557
F1 K1 F1 51.63(19) 6_557 8_557
F1 K1 F3 92.42(13) . 8_557
F1 K1 F3 92.42(13) 11 8_557
F1 K1 F4 71.47(14) 11 8_556
F1 K1 F4 126.36(16) . 8_556
F1 K1 F4 71.47(14) . 6_556
F1 K1 F4 126.36(16) 11 6_556
F1 K1 O1 98.16(14) . 8_556
F1 K1 O1 98.16(14) 11 8_556
F1 K1 O1 147.32(16) 6_557 8_556
F1 K1 O1 147.32(16) 8_557 8_556
F3 K1 V1 35.14(12) 8_557 8_557
F3 K1 V2 35.47(12) 8_557 8_557
F3 K1 K2 50.10(3) 8_557 .
F3 K1 K2 50.10(3) 8_557 8_557
F3 K1 F1 53.23(14) 8_557 6_557
F3 K1 F1 53.23(14) 8_557 8_557
F3 K1 F4 54.78(13) 8_557 6_556
F3 K1 F4 54.78(13) 8_557 8_556
F3 K1 O1 110.9(2) 8_557 8_556
F4 K1 V1 85.19(10) 6_556 8_557
F4 K1 V1 85.19(10) 8_556 8_557
F4 K1 V2 30.63(8) 8_556 8_557
F4 K1 V2 30.63(8) 6_556 8_557
F4 K1 K2 43.86(8) 6_556 .
F4 K1 K2 89.33(10) 6_556 8_557
F4 K1 K2 89.33(10) 8_556 .
F4 K1 K2 43.86(8) 8_556 8_557
F4 K1 F1 84.63(13) 8_556 8_557
F4 K1 F1 84.63(13) 6_556 6_557
F4 K1 F1 108.00(14) 8_556 6_557
F4 K1 F1 108.00(14) 6_556 8_557
F4 K1 F4 55.08(17) 6_556 8_556
F4 K1 O1 64.95(18) 8_556 8_556
F4 K1 O1 64.95(18) 6_556 8_556
O1 K1 V1 146.1(2) 8_556 8_557
O1 K1 V2 75.4(2) 8_556 8_557
O1 K1 K2 103.53(12) 8_556 .
O1 K1 K2 103.52(12) 8_556 8_557
F1 K2 F1 57.5(2) . 6_557
F1 K2 F2 108.70(15) . 6_557
F1 K2 F2 108.70(15) 6_557 .
F1 K2 F2 51.76(14) . .
F1 K2 F2 51.77(14) 6_557 6_557
F1 K2 F3 79.87(14) . 8_557
F1 K2 F3 50.55(15) 6_557 8_557
F1 K2 F3 50.55(15) . .
F1 K2 F3 79.87(15) 6_557 .
F1 K2 F4 86.92(14) . 1_556
F1 K2 F4 67.72(14) 6_557 1_556
F1 K2 F4 67.72(14) . 6_556
F1 K2 F4 86.92(14) 6_557 6_556
F1 K2 F5 117.23(12) . 8_557
F1 K2 F5 99.75(13) . 10
F1 K2 F5 117.23(12) 6_557 10
F1 K2 F5 99.75(13) 6_557 8_557
F2 K2 F2 160.4(2) 6_557 .
F2 K2 F3 50.11(14) 6_557 8_557
F2 K2 F3 50.11(14) . .
F2 K2 F3 118.95(15) 6_557 .
F2 K2 F3 118.95(15) . 8_557
F2 K2 F5 117.85(13) . 8_557
F2 K2 F5 69.78(14) 6_557 8_557
F2 K2 F5 69.78(14) . 10
F2 K2 F5 117.85(13) 6_557 10
F3 K2 F3 124.9(2) 8_557 .
F4 K2 F2 75.17(12) 1_556 6_557
F4 K2 F2 99.91(11) 6_556 6_557
F4 K2 F2 75.17(12) 6_556 .
F4 K2 F2 99.91(11) 1_556 .
F4 K2 F3 50.90(13) 1_556 .
F4 K2 F3 113.72(14) 1_556 8_557
F4 K2 F3 50.90(13) 6_556 8_557
F4 K2 F3 113.72(15) 6_556 .
F4 K2 F4 151.4(2) 6_556 1_556
F4 K2 F5 52.15(12) 6_556 8_557
F4 K2 F5 142.19(11) 1_556 8_557
F4 K2 F5 142.19(11) 6_556 10
F4 K2 F5 52.15(12) 1_556 10
F5 K2 F3 165.73(13) 8_557 .
F5 K2 F3 50.33(14) 8_557 8_557
F5 K2 F3 165.73(13) 10 8_557
F5 K2 F3 50.33(14) 10 .
F5 K2 F5 138.11(17) 10 8_557
F7 K2 F1 115.51(14) 6_557 6_557
F7 K2 F1 161.83(13) . 6_557
F7 K2 F1 161.83(13) 6_557 .
F7 K2 F1 115.51(14) . .
F7 K2 F2 128.58(14) . 6_557
F7 K2 F2 69.16(13) 6_557 6_557
F7 K2 F2 128.58(14) 6_557 .
F7 K2 F2 69.16(13) . .
F7 K2 F3 109.14(14) . .
F7 K2 F3 113.61(14) 6_557 .
F7 K2 F3 113.61(14) . 8_557
F7 K2 F3 109.14(14) 6_557 8_557
F7 K2 F4 75.04(13) 6_557 1_556
F7 K2 F4 75.04(13) . 6_556
F7 K2 F4 130.30(12) . 1_556
F7 K2 F4 130.30(12) 6_557 6_556
F7 K2 F5 67.53(13) 6_557 10
F7 K2 F5 79.59(12) . 10
F7 K2 F5 67.53(13) . 8_557
F7 K2 F5 79.59(12) 6_557 8_557
F7 K2 F7 76.12(16) . 6_557
V3 K3 V3 70.24(5) 7_666 .
V3 K3 K2 123.53(4) . 1_554
V3 K3 K2 68.74(3) 7_666 1_554
F2 K3 V3 77.12(12) . .
F2 K3 V3 77.12(12) 6_556 7_666
F2 K3 V3 145.38(13) . 7_666
F2 K3 V3 145.39(13) 6_556 .
F2 K3 K2 124.24(12) . 1_554
F2 K3 K2 49.63(12) 6_556 1_554
F2 K3 F2 137.0(3) 6_556 .
F2 K3 F4 83.90(14) . 6_556
F2 K3 F4 77.96(14) 6_556 6_556
F2 K3 F4 77.96(14) . .
F2 K3 F4 83.90(14) 6_556 .
F2 K3 F6 111.52(13) . .
F2 K3 F6 111.52(13) 6_556 .
F2 K3 F7 73.46(15) 6_556 6_556
F2 K3 F7 136.53(15) 6_556 .
F2 K3 F7 73.46(15) . .
F2 K3 F7 136.53(15) . 6_556
F2 K3 F8 154.55(15) . 8_556
F2 K3 F8 62.39(14) 6_556 8_556
F2 K3 F8 154.55(15) 6_556 10
F2 K3 F8 62.39(14) . 10
F4 K3 V3 105.77(9) . 7_666
F4 K3 V3 115.49(10) 6_556 7_666
F4 K3 V3 105.77(9) 6_556 .
F4 K3 V3 115.49(10) . .
F4 K3 K2 126.23(9) 6_556 1_554
F4 K3 K2 46.32(9) . 1_554
F4 K3 F4 129.2(2) . 6_556
F4 K3 F6 115.42(10) 6_556 .
F4 K3 F6 115.42(10) . .
F4 K3 F7 139.17(12) . .
F4 K3 F7 139.17(12) 6_556 6_556
F4 K3 F7 76.08(12) . 6_556
F4 K3 F7 76.08(12) 6_556 .
F4 K3 F8 125.80(12) 6_556 10
F4 K3 F8 85.95(12) 6_556 8_556
F4 K3 F8 125.80(12) . 8_556
F4 K3 F8 85.95(12) . 10
F6 K3 V3 35.12(3) . 7_666
F6 K3 V3 35.12(3) . .
F6 K3 K2 96.66(3) . 1_554
F7 K3 V3 83.41(9) . 7_666
F7 K3 V3 29.70(8) . .
F7 K3 V3 83.41(9) 6_556 .
F7 K3 V3 29.70(8) 6_556 7_666
F7 K3 K2 149.66(9) . 1_554
F7 K3 K2 43.65(8) 6_556 1_554
F7 K3 F6 53.05(8) . .
F7 K3 F6 53.05(8) 6_556 .
F7 K3 F7 106.10(16) . 6_556
F7 K3 F8 81.47(12) 6_556 10
F7 K3 F8 81.47(12) . 8_556
F7 K3 F8 55.10(12) 6_556 8_556
F7 K3 F8 55.10(12) . 10
F8 K3 V3 83.32(9) 8_556 .
F8 K3 V3 30.23(8) 10 .
F8 K3 V3 83.32(9) 10 7_666
F8 K3 V3 30.23(8) 8_556 7_666
F8 K3 K2 80.27(8) 8_556 1_554
F8 K3 K2 107.94(8) 10 1_554
F8 K3 F6 53.19(8) 10 .
F8 K3 F6 53.19(8) 8_556 .
F8 K3 F8 106.37(16) 10 8_556
V3 K4 V3 68.58(5) 7_667 1_556
F5 K4 V3 98.09(11) 10 7_667
F5 K4 V3 98.09(11) 2_665 7_667
F5 K4 V3 121.52(10) 10 1_556
F5 K4 V3 121.52(10) 2_665 1_556
F5 K4 F5 116.58(19) 10 2_665
F5 K4 F6 113.75(10) 10 1_556
F5 K4 F6 113.75(10) 2_665 1_556
F5 K4 F7 115.01(13) 2_665 6_557
F5 K4 F7 115.01(13) 10 7_667
F5 K4 F7 69.40(12) 2_665 7_667
F5 K4 F7 69.40(12) 10 6_557
F5 K4 F8 147.82(12) 2_665 10_556
F5 K4 F8 95.08(12) 10 10_556
F5 K4 F8 95.08(12) 2_665 2_666
F5 K4 F8 147.82(12) 10 2_666
F5 K4 O2 48.22(18) 2_665 2_665
F5 K4 O2 144.09(18) 10 2_665
F5 K4 O2 144.09(18) 2_665 .
F5 K4 O2 48.22(18) 10 .
F5 K4 O3 59.78(10) 2_665 .
F5 K4 O3 59.78(10) 10 .
F6 K4 V3 34.10(3) 1_556 1_556
F6 K4 V3 34.48(3) 1_556 7_667
F6 K4 O2 101.69(15) 1_556 2_665
F6 K4 O2 101.69(15) 1_556 .
F7 K4 V3 29.14(7) 6_557 7_667
F7 K4 V3 80.90(9) 7_667 1_556
F7 K4 V3 80.90(9) 6_557 1_556
F7 K4 V3 29.14(7) 7_667 7_667
F7 K4 F6 51.52(8) 7_667 1_556
F7 K4 F6 51.52(8) 6_557 1_556
F7 K4 F7 54.16(14) 6_557 7_667
F7 K4 F8 103.52(12) 7_667 10_556
F7 K4 F8 103.52(12) 6_557 2_666
F7 K4 F8 80.11(12) 7_667 2_666
F7 K4 F8 80.11(12) 6_557 10_556
F7 K4 O2 91.17(17) 7_667 2_665
F7 K4 O2 144.12(17) 6_557 2_665
F7 K4 O2 91.17(17) 6_557 .
F7 K4 O2 144.12(17) 7_667 .
F7 K4 O3 78.98(15) 6_557 .
F7 K4 O3 78.98(15) 7_667 .
F8 K4 V3 81.99(9) 10_556 7_667
F8 K4 V3 29.05(8) 2_666 1_556
F8 K4 V3 81.99(9) 2_666 7_667
F8 K4 V3 29.05(8) 10_556 1_556
F8 K4 F6 52.01(8) 2_666 1_556
F8 K4 F6 52.01(8) 10_556 1_556
F8 K4 F8 52.90(16) 10_556 2_666
F8 K4 O2 102.46(17) 10_556 2_665
F8 K4 O2 56.15(16) 2_666 2_665
F8 K4 O2 102.46(17) 2_666 .
F8 K4 O2 56.15(16) 10_556 .
F8 K4 O3 151.80(10) 10_556 .
F8 K4 O3 151.80(10) 2_666 .
O2 K4 V3 85.02(15) 2_665 1_556
O2 K4 V3 85.02(15) . 1_556
O2 K4 V3 115.09(15) 2_665 7_667
O2 K4 V3 115.09(15) . 7_667
O2 K4 O2 120.4(3) . 2_665
O3 K4 V3 88.80(15) . 7_667
O3 K4 V3 157.37(16) . 1_556
O3 K4 F6 123.27(16) . 1_556
O3 K4 O2 105.58(16) . .
O3 K4 O2 105.58(16) . 2_665
F1D K5 F3 173.9(12) . .
F1D K5 O2 73.8(13) . 1_554
F1D K5 O3 78.4(5) . 3_565
F1D K5 O3 78.4(5) . .
F2 K5 F1D 135.2(9) . .
F2 K5 F1D 135.2(9) 10 .
F2 K5 F2 54.6(2) . 10
F2 K5 F2D 149.3(6) . .
F2 K5 F2D 149.3(6) 10 .
F2 K5 F3 49.61(13) . .
F2 K5 F3 49.61(13) 10 .
F2 K5 F5 99.59(16) 10 10
F2 K5 F5 75.33(16) . 10
F2 K5 F5 75.33(16) 10 .
F2 K5 F5 99.59(16) . .
F2 K5 O2 71.6(2) . 1_554
F2 K5 O2 71.6(2) 10 1_554
F2 K5 O3 86.68(15) . .
F2 K5 O3 139.84(15) 10 .
F2 K5 O3 86.68(15) 10 3_565
F2 K5 O3 139.84(15) . 3_565
F2D K5 F1D 51.8(19) . .
F2D K5 F3 122.1(14) . .
F2D K5 O2 125.5(14) . 1_554
F2D K5 O3 64.31(18) . .
F2D K5 O3 64.31(19) . 3_565
F5 K5 F1D 125.0(10) . .
F5 K5 F1D 125.0(10) 10 .
F5 K5 F2D 79.7(13) 10 .
F5 K5 F2D 79.7(13) . .
F5 K5 F3 49.98(13) 10 .
F5 K5 F3 49.98(13) . .
F5 K5 F5 54.54(17) 10 .
F5 K5 O2 144.30(17) . 1_554
F5 K5 O2 144.30(16) 10 1_554
F5 K5 O3 55.70(13) 10 .
F5 K5 O3 104.98(15) . .
F5 K5 O3 104.98(15) 10 3_565
F5 K5 O3 55.70(13) . 3_565
F8 K5 F1D 76.6(6) . .
F8 K5 F1D 76.6(6) 10 .
F8 K5 F2 61.73(13) 10 .
F8 K5 F2 61.72(13) . 10
F8 K5 F2 108.24(16) . .
F8 K5 F2 108.24(16) 10 10
F8 K5 F2D 102.4(7) 10 .
F8 K5 F2D 102.5(7) . .
F8 K5 F3 106.25(12) 10 .
F8 K5 F3 106.25(12) . .
F8 K5 F5 146.84(13) . 10
F8 K5 F5 92.89(12) 10 10
F8 K5 F5 146.84(13) 10 .
F8 K5 F5 92.89(12) . .
F8 K5 F8 118.27(18) 10 .
F8 K5 O2 59.73(9) . 1_554
F8 K5 O2 59.73(9) 10 1_554
F8 K5 O3 50.49(14) 10 .
F8 K5 O3 154.64(16) 10 3_565
F8 K5 O3 50.49(14) . 3_565
F8 K5 O3 154.64(17) . .
O2 K5 F3 112.4(2) 1_554 .
O2 K5 O3 108.80(13) 1_554 .
O2 K5 O3 108.81(13) 1_554 3_565
O3 K5 F3 99.04(12) 3_565 .
O3 K5 F3 99.04(12) . .
O3 K5 O3 127.5(2) . 3_565
V1 F1 K1 99.6(2) . 9_557
V1 F1 K1 143.0(3) . .
V1 F1 K2 108.1(2) . .
K1 F1 K1 105.34(18) . 9_557
K1 F1 K2 98.84(16) . .
K2 F1 K1 90.10(15) . 9_557
K5 F1D K5 102.2(15) 2_665 .
K5 F1D K5 102.2(15) 3_565 .
K5 F1D K5 102.2(15) 3_565 2_665
V1 F2 K2 100.9(2) . .
V1 F2 K3 128.7(3) . .
V1 F2 K5 105.5(2) . .
K3 F2 K2 88.35(15) . .
K3 F2 K5 119.77(19) . .
K5 F2 K2 107.10(18) . .
K5 F2D K5 102.5(17) 2_665 .
K5 F2D K5 102.5(17) 3_565 .
K5 F2D K5 102.5(17) 3_565 2_665
V1 F3 K1 97.0(2) . 9_557
V1 F3 K2 89.93(10) . 9_557
V1 F3 K2 89.93(11) . .
V1 F3 K5 84.25(18) . .
V2 F3 V1 168.4(3) . .
V2 F3 K1 94.6(2) . 9_557
V2 F3 K2 90.60(11) . .
V2 F3 K2 90.60(11) . 9_557
V2 F3 K5 84.18(19) . .
K1 F3 K2 87.34(11) 9_557 9_557
K1 F3 K2 87.34(11) 9_557 .
K1 F3 K5 178.7(2) 9_557 .
K2 F3 K2 174.6(2) 9_557 .
K2 F3 K5 92.67(11) . .
K2 F3 K5 92.67(11) 9_557 .
V2 F4 K1 98.01(16) 1_554 9_556
V2 F4 K2 106.15(16) 1_554 1_554
V2 F4 K3 134.5(2) 1_554 .
K2 F4 K1 92.13(13) 1_554 9_556
K3 F4 K1 123.91(16) . 9_556
K3 F4 K2 90.36(12) . 1_554
V2 F5 K2 99.64(18) . 9_557
V2 F5 K4 115.0(2) . 3_565
V2 F5 K5 103.87(18) . .
K4 F5 K2 107.71(15) 3_565 9_557
K4 F5 K5 122.28(17) 3_565 .
K5 F5 K2 105.73(15) . 9_557
V3 F6 V3 180.0 7_666 .
V3 F6 K3 90.00(4) . 7_666
V3 F6 K3 90.00(4) 7_666 7_666
V3 F6 K3 90.000(1) 7_666 .
V3 F6 K3 90.00(4) . .
V3 F6 K4 89.41(5) 7_666 1_554
V3 F6 K4 90.59(5) . 1_554
V3 F6 K4 89.41(5) . 7_667
V3 F6 K4 90.59(5) 7_666 7_667
K3 F6 K3 180.00(6) . 7_666
K3 F6 K4 90.00(4) . 1_554
K3 F6 K4 90.00(4) 7_666 1_554
K3 F6 K4 90.00(4) 7_666 7_667
K3 F6 K4 90.00(4) . 7_667
K4 F6 K4 180.0 7_667 1_554
V3 F7 K2 139.3(2) . .
V3 F7 K3 101.57(16) . .
V3 F7 K4 101.87(15) . 7_667
K2 F7 K3 91.03(11) . .
K2 F7 K4 114.41(14) . 7_667
K3 F7 K4 98.52(13) . 7_667
V3 F8 K3 99.39(16) 3_565 9_556
V3 F8 K4 102.55(16) 3_565 3_564
V3 F8 K5 112.91(18) 3_565 .
K3 F8 K4 97.17(12) 9_556 3_564
K5 F8 K3 115.23(15) . 9_556
K5 F8 K4 125.56(16) . 3_564
V1 O1 K1 165.8(5) . 9_556
V2 O2 K4 98.0(3) . 3_565
V2 O2 K4 98.0(3) . .
V2 O2 K5 151.9(6) . 1_556
K4 O2 K4 108.6(3) . 3_565
K5 O2 K4 98.3(2) 1_556 3_565
K5 O2 K4 98.3(2) 1_556 .
V3 O3 K4 146.9(4) . .
V3 O3 K5 98.7(2) . 2_665
V3 O3 K5 98.7(2) . .
K4 O3 K5 102.85(15) . 2_665
K4 O3 K5 102.85(15) . .
K5 O3 K5 97.9(2) . 2_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
V1 F1 1.797(5) .
V1 F1 1.797(5) 10
V1 F2 1.842(5) .
V1 F2 1.842(5) 10
V1 F3 2.134(6) .
V1 O1 1.574(9) .
V2 F3 2.083(6) .
V2 F4 1.841(4) 10_556
V2 F4 1.841(4) 1_556
V2 F5 1.834(4) .
V2 F5 1.834(4) 10
V2 O2 1.560(9) .
V3 F6 2.0756(14) .
V3 F7 1.824(4) 12_665
V3 F7 1.825(4) .
V3 F8 1.841(4) 10
V3 F8 1.841(4) 2_665
V3 O3 1.588(6) .
K1 F1 2.924(6) 8_557
K1 F1 2.924(6) 6_557
K1 F1 2.529(4) 11
K1 F1 2.529(4) .
K1 F3 2.749(6) 8_557
K1 F4 2.822(5) 8_556
K1 F4 2.822(5) 6_556
K1 O1 2.971(9) 8_556
K2 F1 2.811(5) .
K2 F1 2.811(5) 6_557
K2 F2 2.966(5) .
K2 F2 2.966(5) 6_557
K2 F3 3.118(8) 8_557
K2 F3 3.118(6) .
K2 F4 2.815(4) 6_556
K2 F4 2.815(4) 1_556
K2 F5 2.998(5) 8_557
K2 F5 2.998(5) 10
K2 F7 2.687(4) .
K2 F7 2.687(4) 6_557
K3 F2 2.607(5) .
K3 F2 2.607(5) 6_556
K3 F4 2.671(4) .
K3 F4 2.671(4) 6_556
K3 F6 2.9512(19) .
K3 F7 2.768(4) 6_556
K3 F7 2.768(4) .
K3 F8 2.817(4) 10
K3 F8 2.817(4) 8_556
K4 F5 2.740(5) 2_665
K4 F5 2.740(5) 10
K4 F6 3.044(2) 1_556
K4 F7 2.827(4) 7_667
K4 F7 2.827(4) 6_557
K4 F8 2.836(4) 10_556
K4 F8 2.836(4) 2_666
K4 O2 3.351(6) 2_665
K4 O2 3.351(6) .
K4 O3 2.964(7) .
K5 F1D 3.14(3) .
K5 F2 2.782(6) 10
K5 F2 2.782(6) .
K5 F2D 3.13(4) .
K5 F3 3.275(6) .
K5 F5 2.802(5) .
K5 F5 2.802(5) 10
K5 F8 2.704(4) 10
K5 F8 2.704(4) .
K5 O2 3.162(9) 1_554
K5 O3 3.240(5) 3_565
K5 O3 3.240(5) .
F1 K1 2.924(6) 9_557
F1D K5 3.14(3) 2_665
F1D K5 3.14(3) 3_565
F2D K5 3.13(4) 2_665
F2D K5 3.13(4) 3_565
F3 K1 2.749(6) 9_557
F3 K2 3.118(6) 9_557
F4 V2 1.841(4) 1_554
F4 K1 2.822(5) 9_556
F4 K2 2.815(4) 1_554
F5 K2 2.998(5) 9_557
F5 K4 2.740(5) 3_565
F6 V3 2.0756(14) 7_666
F6 K3 2.9513(19) 7_666
F6 K4 3.044(2) 1_554
F6 K4 3.044(2) 7_667
F7 K4 2.827(4) 7_667
F8 V3 1.841(4) 3_565
F8 K3 2.817(4) 9_556
F8 K4 2.836(4) 3_564
O1 K1 2.971(9) 9_556
O2 K4 3.351(6) 3_565
O2 K5 3.162(9) 1_556
O3 K5 3.240(5) 2_665
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
V1 K1 F1 V1 -178.2(4) 8_557 .
V1 K1 F1 K1 -47.47(15) 8_557 9_557
V1 K1 F1 K2 45.08(14) 8_557 .
V2 K1 F1 V1 111.9(4) 8_557 .
V2 K1 F1 K1 -117.36(14) 8_557 9_557
V2 K1 F1 K2 -24.81(16) 8_557 .
V3 K3 F2 V1 -175.6(3) . .
V3 K3 F2 V1 164.80(17) 7_666 .
V3 K3 F2 K2 -92.6(2) 7_666 .
V3 K3 F2 K2 -72.92(10) . .
V3 K3 F2 K5 35.88(18) . .
V3 K3 F2 K5 16.3(4) 7_666 .
V3 K3 F4 V2 -0.4(3) . 1_554
V3 K3 F4 V2 -75.6(3) 7_666 1_554
V3 K3 F4 K1 -154.19(13) . 9_556
V3 K3 F4 K1 130.56(15) 7_666 9_556
V3 K3 F4 K2 113.01(10) . 1_554
V3 K3 F4 K2 37.75(13) 7_666 1_554
V3 K3 F6 V3 180.0 . 7_666
V3 K3 F6 V3 180.0 7_666 .
V3 K3 F6 K4 89.41(5) . 7_667
V3 K3 F6 K4 -90.59(5) 7_666 7_667
V3 K3 F6 K4 89.41(5) 7_666 1_554
V3 K3 F6 K4 -90.59(5) . 1_554
V3 K3 F7 V3 61.02(15) 7_666 .
V3 K3 F7 K2 141.1(2) . .
V3 K3 F7 K2 -157.91(10) 7_666 .
V3 K3 F7 K4 -43.04(8) 7_666 7_667
V3 K3 F7 K4 -104.06(18) . 7_667
V3 K4 O2 V2 -132.3(3) 1_556 .
V3 K4 O2 V2 -68.8(4) 7_667 .
V3 K4 O2 K4 126.4(2) 1_556 3_565
V3 K4 O2 K4 -170.03(14) 7_667 3_565
V3 K4 O2 K5 88.3(2) 7_667 1_556
V3 K4 O2 K5 24.76(18) 1_556 1_556
V3 K4 O3 V3 0.000(3) 7_667 .
V3 K4 O3 V3 0.000(7) 1_556 .
V3 K4 O3 K5 129.34(13) 1_556 .
V3 K4 O3 K5 -129.34(13) 1_556 2_665
V3 K4 O3 K5 129.34(13) 7_667 .
V3 K4 O3 K5 -129.34(13) 7_667 2_665
K1 V1 F1 K1 132.2(5) 9_557 .
K1 V1 F1 K2 -93.3(2) 9_557 .
K1 V1 F2 K2 18.1(2) 9_557 .
K1 V1 F2 K3 114.7(3) 9_557 .
K1 V1 F2 K5 -93.29(19) 9_557 .
K1 V1 F3 V2 180.0(15) 9_557 .
K1 V1 F3 K2 87.32(11) 9_557 .
K1 V1 F3 K2 -87.31(11) 9_557 9_557
K1 V1 F3 K5 180.0 9_557 .
K1 V1 O1 K1 179.993(16) 9_557 9_556
K1 V2 F3 V1 -180.0(15) 9_557 .
K1 V2 F3 K2 -87.38(11) 9_557 .
K1 V2 F3 K2 87.38(11) 9_557 9_557
K1 V2 F3 K5 180.0 9_557 .
K1 V2 F5 K2 13.90(19) 9_557 9_557
K1 V2 F5 K4 128.70(16) 9_557 3_565
K1 V2 F5 K5 -95.08(17) 9_557 .
K1 V2 O2 K4 -124.91(19) 9_557 3_565
K1 V2 O2 K4 124.91(19) 9_557 .
K1 V2 O2 K5 0.001(10) 9_557 1_556
K2 V1 F1 K1 0.2(2) 9_557 9_557
K2 V1 F1 K1 93.3(2) . 9_557
K2 V1 F1 K1 -134.5(6) . .
K2 V1 F1 K1 132.4(4) 9_557 .
K2 V1 F1 K2 -93.08(19) 9_557 .
K2 V1 F2 K2 93.35(17) 9_557 .
K2 V1 F2 K3 96.7(3) . .
K2 V1 F2 K3 -169.97(19) 9_557 .
K2 V1 F2 K5 -111.4(2) . .
K2 V1 F2 K5 -18.0(3) 9_557 .
K2 V1 F3 V2 -92.7(14) 9_557 .
K2 V1 F3 V2 92.7(14) . .
K2 V1 F3 K1 87.31(11) 9_557 9_557
K2 V1 F3 K1 -87.32(11) . 9_557
K2 V1 F3 K2 174.6(2) 9_557 .
K2 V1 F3 K2 -174.6(2) . 9_557
K2 V1 F3 K5 92.69(11) . .
K2 V1 F3 K5 -92.69(11) 9_557 .
K2 V1 O1 K1 92.9(19) 9_557 9_556
K2 V1 O1 K1 -92.9(19) . 9_556
K2 V2 F3 V1 92.6(14) 9_557 .
K2 V2 F3 V1 -92.6(14) . .
K2 V2 F3 K1 -87.38(11) 9_557 9_557
K2 V2 F3 K1 87.38(11) . 9_557
K2 V2 F3 K2 -174.8(2) 9_557 .
K2 V2 F3 K2 174.8(2) . 9_557
K2 V2 F3 K5 92.62(11) 9_557 .
K2 V2 F3 K5 -92.62(11) . .
K2 V2 F5 K2 92.91(16) . 9_557
K2 V2 F5 K4 114.8(2) 9_557 3_565
K2 V2 F5 K4 -152.29(12) . 3_565
K2 V2 F5 K5 -16.1(2) . .
K2 V2 F5 K5 -109.0(2) 9_557 .
K2 V2 O2 K4 -37.6(5) 9_557 3_565
K2 V2 O2 K4 147.78(10) . 3_565
K2 V2 O2 K4 37.6(5) . .
K2 V2 O2 K4 -147.78(10) 9_557 .
K2 V2 O2 K5 87.3(3) 9_557 1_556
K2 V2 O2 K5 -87.3(3) . 1_556
K2 K1 F1 V1 159.6(3) 8_557 .
K2 K1 F1 V1 136.7(5) . .
K2 K1 F1 K1 -92.55(19) . 9_557
K2 K1 F1 K1 -69.7(3) 8_557 9_557
K2 K1 F1 K2 22.9(3) 8_557 .
K2 K3 F2 V1 62.4(4) 1_554 .
K2 K3 F2 K2 165.09(8) 1_554 .
K2 K3 F2 K5 -86.1(2) 1_554 .
K2 K3 F4 V2 -113.4(3) 1_554 1_554
K2 K3 F4 K1 92.81(19) 1_554 9_556
K2 K3 F6 V3 -36.81(4) 1_554 7_666
K2 K3 F6 V3 143.18(4) 1_554 .
K2 K3 F6 K4 -127.41(4) 1_554 7_667
K2 K3 F6 K4 52.59(4) 1_554 1_554
K2 K3 F7 V3 37.9(3) 1_554 .
K2 K3 F7 K2 179.00(6) 1_554 .
K2 K3 F7 K4 -66.1(2) 1_554 7_667
K3 V1 F1 K1 -75.3(4) . .
K3 V1 F1 K1 56.6(9) 9_556 .
K3 V1 F1 K1 152.54(16) . 9_557
K3 V1 F1 K1 -75.6(7) 9_556 9_557
K3 V1 F1 K2 59.26(16) . .
K3 V1 F1 K2 -168.9(5) 9_556 .
K3 V1 F2 K2 157.62(10) 9_556 .
K3 V1 F2 K2 -96.7(3) . .
K3 V1 F2 K3 -105.7(3) 9_556 .
K3 V1 F2 K5 152.0(4) . .
K3 V1 F2 K5 46.3(2) 9_556 .
K3 V1 F3 V2 60.1(14) . .
K3 V1 F3 V2 -60.1(14) 9_556 .
K3 V1 F3 K1 -119.91(5) . 9_557
K3 V1 F3 K1 119.91(5) 9_556 9_557
K3 V1 F3 K2 -32.60(15) . .
K3 V1 F3 K2 -152.78(8) 9_556 .
K3 V1 F3 K2 32.60(15) 9_556 9_557
K3 V1 F3 K2 152.78(8) . 9_557
K3 V1 F3 K5 60.09(5) . .
K3 V1 F3 K5 -60.09(5) 9_556 .
K3 V1 O1 K1 -60.0(18) . 9_556
K3 V1 O1 K1 60.0(18) 9_556 9_556
K3 V3 K3 V3 0.0 7_666 7_666
K3 V3 K3 K2 -45.56(5) 7_666 1_554
K3 V3 K3 F2 -168.30(13) 7_666 .
K3 V3 K3 F2 20.4(2) 7_666 6_556
K3 V3 K3 F4 -98.55(11) 7_666 .
K3 V3 K3 F4 111.95(11) 7_666 6_556
K3 V3 K3 F6 0.0 7_666 .
K3 V3 K3 F7 112.57(18) 7_666 .
K3 V3 K3 F7 -27.42(9) 7_666 6_556
K3 V3 K3 F8 -111.78(16) 7_666 10
K3 V3 K3 F8 28.08(8) 7_666 8_556
K3 V3 F6 K3 180.0 . 7_666
K3 V3 F6 K3 180.0 7_666 .
K3 V3 F6 K4 -90.00(4) . 7_667
K3 V3 F6 K4 90.00(3) . 1_554
K3 V3 F6 K4 90.00(4) 7_666 7_667
K3 V3 F6 K4 -90.00(4) 7_666 1_554
K3 V3 F7 K2 -105.4(3) . .
K3 V3 F7 K2 163.51(19) 7_666 .
K3 V3 F7 K3 -91.05(14) 7_666 .
K3 V3 F7 K4 10.35(17) 7_666 7_667
K3 V3 F7 K4 101.40(17) . 7_667
K3 V3 O3 K4 -90.28(19) 7_666 .
K3 V3 O3 K4 90.3(2) . .
K3 V3 O3 K5 -40.0(3) . .
K3 V3 O3 K5 40.0(3) 7_666 2_665
K3 V3 O3 K5 -139.42(9) . 2_665
K3 V3 O3 K5 139.42(9) 7_666 .
K4 V2 F3 V1 -55.1(15) . .
K4 V2 F3 V1 55.2(15) 3_565 .
K4 V2 F3 K1 -124.85(10) 3_565 9_557
K4 V2 F3 K1 124.86(10) . 9_557
K4 V2 F3 K2 37.47(19) . .
K4 V2 F3 K2 -37.5(2) 3_565 9_557
K4 V2 F3 K2 147.76(7) 3_565 .
K4 V2 F3 K2 -147.76(7) . 9_557
K4 V2 F3 K5 -55.15(10) . .
K4 V2 F3 K5 55.15(10) 3_565 .
K4 V2 F5 K2 172.14(9) . 9_557
K4 V2 F5 K2 -114.8(2) 3_565 9_557
K4 V2 F5 K4 -73.06(19) . 3_565
K4 V2 F5 K5 136.2(3) 3_565 .
K4 V2 F5 K5 63.16(17) . .
K4 V2 O2 K4 -110.2(4) 3_565 .
K4 V2 O2 K4 110.2(4) . 3_565
K4 V2 O2 K5 -124.9(10) . 1_556
K4 V2 O2 K5 124.9(10) 3_565 1_556
K4 V3 K3 V3 -61.22(4) 7_667 7_666
K4 V3 K3 V3 60.48(4) 1_554 7_666
K4 V3 K3 K2 -106.78(5) 7_667 1_554
K4 V3 K3 K2 14.92(4) 1_554 1_554
K4 V3 K3 F2 80.8(2) 1_554 6_556
K4 V3 K3 F2 -40.9(2) 7_667 6_556
K4 V3 K3 F2 -107.82(13) 1_554 .
K4 V3 K3 F2 130.48(13) 7_667 .
K4 V3 K3 F4 -38.07(11) 1_554 .
K4 V3 K3 F4 -159.77(11) 7_667 .
K4 V3 K3 F4 172.43(11) 1_554 6_556
K4 V3 K3 F4 50.73(11) 7_667 6_556
K4 V3 K3 F6 60.48(4) 1_554 .
K4 V3 K3 F6 -61.22(4) 7_667 .
K4 V3 K3 F7 173.05(18) 1_554 .
K4 V3 K3 F7 -88.64(9) 7_667 6_556
K4 V3 K3 F7 33.06(9) 1_554 6_556
K4 V3 K3 F7 51.35(17) 7_667 .
K4 V3 K3 F8 -33.14(8) 7_667 8_556
K4 V3 K3 F8 -51.30(16) 1_554 10
K4 V3 K3 F8 -173.00(16) 7_667 10
K4 V3 K3 F8 88.56(9) 1_554 8_556
K4 V3 F6 K3 90.00(3) 7_667 .
K4 V3 F6 K3 90.00(3) 1_554 7_666
K4 V3 F6 K3 -90.00(4) 7_667 7_666
K4 V3 F6 K3 -90.00(4) 1_554 .
K4 V3 F6 K4 180.0 7_667 1_554
K4 V3 F6 K4 180.0 1_554 7_667
K4 V3 F7 K2 -113.0(2) 1_554 .
K4 V3 F7 K2 153.2(3) 7_667 .
K4 V3 F7 K3 -7.53(19) 1_554 .
K4 V3 F7 K3 -101.40(17) 7_667 .
K4 V3 F7 K4 93.87(12) 1_554 7_667
K4 V3 O3 K4 180.000(2) 1_554 .
K4 V3 O3 K4 0.000(6) 7_667 .
K4 V3 O3 K5 49.71(14) 1_554 .
K4 V3 O3 K5 -130.29(14) 7_667 .
K4 V3 O3 K5 130.29(14) 7_667 2_665
K4 V3 O3 K5 -49.71(14) 1_554 2_665
K5 V1 F1 K1 90.15(17) . 9_557
K5 V1 F1 K1 -137.7(4) . .
K5 V1 F1 K2 -3.1(3) . .
K5 V1 F2 K2 111.4(2) . .
K5 V1 F2 K3 -152.0(4) . .
K5 V1 F3 V2 0.000(14) . .
K5 V1 F3 K1 180.0 . 9_557
K5 V1 F3 K2 -92.69(11) . .
K5 V1 F3 K2 92.69(11) . 9_557
K5 V1 O1 K1 -0.006(16) . 9_556
K5 V2 F3 V1 0.000(13) . .
K5 V2 F3 K1 180.0 . 9_557
K5 V2 F3 K2 92.62(11) . .
K5 V2 F3 K2 -92.62(11) . 9_557
K5 V2 F5 K2 109.0(2) . 9_557
K5 V2 F5 K4 -136.2(3) . 3_565
K5 V2 O2 K4 55.09(19) . 3_565
K5 V2 O2 K4 -55.09(19) . .
K5 V2 O2 K5 179.999(7) . 1_556
K5 V3 K3 V3 97.70(10) 2_665 7_666
K5 V3 K3 V3 146.00(6) . 7_666
K5 V3 K3 K2 52.14(10) 2_665 1_554
K5 V3 K3 K2 100.44(4) . 1_554
K5 V3 K3 F2 -70.60(15) 2_665 .
K5 V3 K3 F2 166.4(2) . 6_556
K5 V3 K3 F2 -22.30(13) . .
K5 V3 K3 F2 118.1(2) 2_665 6_556
K5 V3 K3 F4 -102.05(11) . 6_556
K5 V3 K3 F4 -0.85(14) 2_665 .
K5 V3 K3 F4 47.45(11) . .
K5 V3 K3 F4 -150.36(13) 2_665 6_556
K5 V3 K3 F6 146.00(6) . .
K5 V3 K3 F6 97.70(10) 2_665 .
K5 V3 K3 F7 70.28(13) 2_665 6_556
K5 V3 K3 F7 -101.43(18) . .
K5 V3 K3 F7 -149.7(2) 2_665 .
K5 V3 K3 F7 118.58(9) . 6_556
K5 V3 K3 F8 174.09(9) . 8_556
K5 V3 K3 F8 -14.09(17) 2_665 10
K5 V3 K3 F8 125.78(12) 2_665 8_556
K5 V3 K3 F8 34.22(16) . 10
K5 V3 F6 K3 40.49(6) 2_665 7_666
K5 V3 F6 K3 139.51(6) . 7_666
K5 V3 F6 K3 -139.51(6) 2_665 .
K5 V3 F6 K3 -40.49(6) . .
K5 V3 F6 K4 130.49(6) 2_665 7_667
K5 V3 F6 K4 49.51(6) . 1_554
K5 V3 F6 K4 -49.51(6) 2_665 1_554
K5 V3 F6 K4 -130.49(6) . 7_667
K5 V3 F7 K2 33.0(5) 2_665 .
K5 V3 F7 K2 -32.1(3) . .
K5 V3 F7 K3 138.4(2) 2_665 .
K5 V3 F7 K3 73.29(12) . .
K5 V3 F7 K4 -120.2(3) 2_665 7_667
K5 V3 F7 K4 174.69(11) . 7_667
K5 V3 O3 K4 130.29(14) . .
K5 V3 O3 K4 -130.29(14) 2_665 .
K5 V3 O3 K5 -99.4(3) . 2_665
K5 V3 O3 K5 99.4(3) 2_665 .
F1 V1 F1 K1 95.0(5) 10 .
F1 V1 F1 K1 -37.2(3) 10 9_557
F1 V1 F1 K2 -130.46(14) 10 .
F1 V1 F2 K2 57.1(8) 10 .
F1 V1 F2 K2 -27.6(2) . .
F1 V1 F2 K3 69.1(3) . .
F1 V1 F2 K3 153.8(6) 10 .
F1 V1 F2 K5 -139.0(2) . .
F1 V1 F2 K5 -54.3(8) 10 .
F1 V1 F3 V2 -134.1(14) 10 .
F1 V1 F3 V2 134.0(14) . .
F1 V1 F3 K1 -45.98(17) . 9_557
F1 V1 F3 K1 45.97(17) 10 9_557
F1 V1 F3 K2 -133.3(2) . 9_557
F1 V1 F3 K2 133.3(2) 10 .
F1 V1 F3 K2 41.34(19) . .
F1 V1 F3 K2 -41.34(19) 10 9_557
F1 V1 F3 K5 134.03(17) . .
F1 V1 F3 K5 -134.03(17) 10 .
F1 V1 O1 K1 -134.1(18) . 9_556
F1 V1 O1 K1 134.1(18) 10 9_556
F1 K1 F1 V1 -161.3(4) 8_557 .
F1 K1 F1 V1 -169.4(4) 6_557 .
F1 K1 F1 V1 -109.0(8) 11 .
F1 K1 F1 K1 -38.60(19) 6_557 9_557
F1 K1 F1 K1 -30.6(3) 8_557 9_557
F1 K1 F1 K1 21.8(8) 11 9_557
F1 K1 F1 K2 114.3(7) 11 .
F1 K1 F1 K2 53.95(13) 6_557 .
F1 K1 F1 K2 62.0(2) 8_557 .
F1 K2 F1 V1 147.1(4) 6_557 .
F1 K2 F1 K1 -58.67(15) 6_557 .
F1 K2 F1 K1 46.88(15) 6_557 9_557
F1 K2 F2 V1 22.15(19) . .
F1 K2 F2 V1 13.8(2) 6_557 .
F1 K2 F2 K3 -107.0(2) . .
F1 K2 F2 K3 -115.35(16) 6_557 .
F1 K2 F2 K5 123.93(16) 6_557 .
F1 K2 F2 K5 132.3(2) . .
F1 K2 F3 V1 -32.61(18) . .
F1 K2 F3 V1 -88.54(19) 6_557 .
F1 K2 F3 V2 158.9(3) . .
F1 K2 F3 V2 103.0(2) 6_557 .
F1 K2 F3 K1 64.41(18) . 9_557
F1 K2 F3 K1 8.48(16) 6_557 9_557
F1 K2 F3 K5 -172.79(17) 6_557 .
F1 K2 F3 K5 -116.9(2) . .
F1 K2 F7 V3 90.8(3) . .
F1 K2 F7 V3 153.6(4) 6_557 .
F1 K2 F7 K3 44.4(5) 6_557 .
F1 K2 F7 K3 -18.41(17) . .
F1 K2 F7 K4 -118.25(15) . 7_667
F1 K2 F7 K4 -55.4(5) 6_557 7_667
F1D K5 F2 V1 -139.2(11) . .
F1D K5 F2 K2 113.9(11) . .
F1D K5 F2 K3 15.8(12) . .
F1D K5 F2D K5 53.0(14) . 3_565
F1D K5 F2D K5 -53.0(14) . 2_665
F1D K5 F5 V2 -131.4(8) . .
F1D K5 F5 K2 124.2(8) . 9_557
F1D K5 F5 K4 0.7(9) . 3_565
F1D K5 F8 V3 -90.8(11) . 3_565
F1D K5 F8 K3 156.0(11) . 9_556
F1D K5 F8 K4 35.5(11) . 3_564
F1D K5 O3 V3 -87.2(12) . .
F1D K5 O3 K4 118.0(12) . .
F1D K5 O3 K5 12.9(11) . 2_665
F2 V1 F1 K1 123.6(2) . 9_557
F2 V1 F1 K1 47.1(8) 10 9_557
F2 V1 F1 K1 179.3(6) 10 .
F2 V1 F1 K1 -104.2(4) . .
F2 V1 F1 K2 30.4(2) . .
F2 V1 F1 K2 -46.2(8) 10 .
F2 V1 F2 K2 133.65(13) 10 .
F2 V1 F2 K3 -129.7(2) 10 .
F2 V1 F2 K5 22.3(3) 10 .
F2 V1 F3 V2 -44.6(14) 10 .
F2 V1 F3 V2 44.5(14) . .
F2 V1 F3 K1 135.44(18) 10 9_557
F2 V1 F3 K1 -135.45(18) . 9_557
F2 V1 F3 K2 -137.2(2) 10 .
F2 V1 F3 K2 48.1(2) 10 9_557
F2 V1 F3 K2 137.2(2) . 9_557
F2 V1 F3 K2 -48.1(2) . .
F2 V1 F3 K5 -44.56(18) 10 .
F2 V1 F3 K5 44.55(18) . .
F2 V1 O1 K1 44.6(19) 10 9_556
F2 V1 O1 K1 -44.5(19) . 9_556
F2 K2 F1 V1 154.9(2) 6_557 .
F2 K2 F1 V1 -23.5(2) . .
F2 K2 F1 K1 -123.72(19) . 9_557
F2 K2 F1 K1 130.7(2) . .
F2 K2 F1 K1 -50.9(2) 6_557 .
F2 K2 F1 K1 54.67(15) 6_557 9_557
F2 K2 F2 V1 17.58(18) 6_557 .
F2 K2 F2 K3 -111.56(13) 6_557 .
F2 K2 F2 K5 127.72(14) 6_557 .
F2 K2 F3 V1 -123.73(18) 6_557 .
F2 K2 F3 V1 36.48(18) . .
F2 K2 F3 V2 67.8(2) 6_557 .
F2 K2 F3 V2 -132.0(3) . .
F2 K2 F3 K1 133.5(2) . 9_557
F2 K2 F3 K1 -26.7(2) 6_557 9_557
F2 K2 F3 K5 152.03(13) 6_557 .
F2 K2 F3 K5 -47.76(16) . .
F2 K2 F7 V3 -122.6(3) 6_557 .
F2 K2 F7 V3 67.0(3) . .
F2 K2 F7 K3 -42.15(13) . .
F2 K2 F7 K3 128.22(13) 6_557 .
F2 K2 F7 K4 28.4(2) 6_557 7_667
F2 K2 F7 K4 -141.99(17) . 7_667
F2 K3 F2 V1 -2.8(3) 6_556 .
F2 K3 F2 K2 99.88(12) 6_556 .
F2 K3 F2 K5 -151.3(2) 6_556 .
F2 K3 F4 V2 -150.3(3) 6_556 1_554
F2 K3 F4 V2 68.9(3) . 1_554
F2 K3 F4 K1 -84.93(19) . 9_556
F2 K3 F4 K1 55.82(19) 6_556 9_556
F2 K3 F4 K2 -36.99(15) 6_556 1_554
F2 K3 F4 K2 -177.74(18) . 1_554
F2 K3 F6 V3 12.27(13) 6_556 7_666
F2 K3 F6 V3 12.27(13) . .
F2 K3 F6 V3 -167.73(13) . 7_666
F2 K3 F6 V3 -167.73(13) 6_556 .
F2 K3 F6 K4 -78.32(13) . 1_554
F2 K3 F6 K4 101.68(13) 6_556 1_554
F2 K3 F6 K4 101.68(13) . 7_667
F2 K3 F6 K4 -78.32(13) 6_556 7_667
F2 K3 F7 V3 124.4(2) 6_556 .
F2 K3 F7 V3 -92.9(2) . .
F2 K3 F7 K2 48.12(15) . .
F2 K3 F7 K2 -94.5(2) 6_556 .
F2 K3 F7 K4 162.99(16) . 7_667
F2 K3 F7 K4 20.3(2) 6_556 7_667
F2 K5 F1D K5 -87(2) . 2_665
F2 K5 F1D K5 -167.7(5) 10 2_665
F2 K5 F1D K5 87(2) 10 3_565
F2 K5 F1D K5 167.7(5) . 3_565
F2 K5 F2 V1 -17.9(3) 10 .
F2 K5 F2 K2 -124.84(11) 10 .
F2 K5 F2 K3 137.05(16) 10 .
F2 K5 F2D K5 169.2(8) . 3_565
F2 K5 F2D K5 -169.2(8) 10 2_665
F2 K5 F2D K5 63(4) . 2_665
F2 K5 F2D K5 -63(4) 10 3_565
F2 K5 F3 V1 36.99(15) 10 .
F2 K5 F3 V1 -36.99(15) . .
F2 K5 F3 V2 -143.01(15) 10 .
F2 K5 F3 V2 143.01(15) . .
F2 K5 F3 K2 126.7(2) 10 .
F2 K5 F3 K2 52.67(15) . .
F2 K5 F3 K2 -126.7(2) . 9_557
F2 K5 F3 K2 -52.67(15) 10 9_557
F2 K5 F5 V2 43.9(2) . .
F2 K5 F5 V2 93.2(2) 10 .
F2 K5 F5 K2 -11.19(14) 10 9_557
F2 K5 F5 K2 -60.47(16) . 9_557
F2 K5 F5 K4 176.05(19) . 3_565
F2 K5 F5 K4 -134.7(2) 10 3_565
F2 K5 F8 V3 106.2(2) 10 3_565
F2 K5 F8 V3 135.66(19) . 3_565
F2 K5 F8 K3 22.39(19) . 9_556
F2 K5 F8 K3 -7.07(15) 10 9_556
F2 K5 F8 K4 -127.5(2) 10 3_564
F2 K5 F8 K4 -98.0(2) . 3_564
F2 K5 O3 V3 64.4(4) 10 .
F2 K5 O3 V3 50.2(2) . .
F2 K5 O3 K4 -90.3(3) 10 .
F2 K5 O3 K4 -104.47(18) . .
F2 K5 O3 K5 150.35(17) . 2_665
F2 K5 O3 K5 164.53(18) 10 2_665
F2D K5 F1D K5 -52.8(12) . 3_565
F2D K5 F1D K5 52.8(12) . 2_665
F2D K5 F2 V1 132(2) . .
F2D K5 F2 K2 25(3) . .
F2D K5 F2 K3 -73(2) . .
F2D K5 F3 V1 180.0 . .
F2D K5 F3 V2 0.0 . .
F2D K5 F3 K2 -90.34(11) . .
F2D K5 F3 K2 90.34(11) . 9_557
F2D K5 F5 V2 -104.9(7) . .
F2D K5 F5 K2 150.7(7) . 9_557
F2D K5 F5 K4 27.2(7) . 3_565
F2D K5 F8 V3 -45.6(13) . 3_565
F2D K5 F8 K3 -158.8(13) . 9_556
F2D K5 F8 K4 80.7(13) . 3_564
F2D K5 O3 V3 -140.2(16) . .
F2D K5 O3 K4 65.1(15) . .
F2D K5 O3 K5 -40.1(16) . 2_665
F3 V1 F1 K1 175.1(5) . .
F3 V1 F1 K1 42.87(16) . 9_557
F3 V1 F1 K2 -50.41(19) . .
F3 V1 F2 K2 52.84(17) . .
F3 V1 F2 K3 149.5(3) . .
F3 V1 F2 K5 -58.51(18) . .
F3 V2 F5 K2 51.37(16) . 9_557
F3 V2 F5 K4 166.2(2) . 3_565
F3 V2 F5 K5 -57.61(18) . .
F3 K1 F1 V1 147.1(4) 8_557 .
F3 K1 F1 K1 -82.1(2) 8_557 9_557
F3 K1 F1 K2 10.43(19) 8_557 .
F3 K2 F1 V1 -163.6(3) 8_557 .
F3 K2 F1 V1 42.3(2) . .
F3 K2 F1 K1 -57.86(16) . 9_557
F3 K2 F1 K1 96.22(14) 8_557 9_557
F3 K2 F1 K1 -9.33(17) 8_557 .
F3 K2 F1 K1 -163.4(3) . .
F3 K2 F2 V1 -44.5(2) . .
F3 K2 F2 V1 68.4(3) 8_557 .
F3 K2 F2 K3 -60.8(2) 8_557 .
F3 K2 F2 K3 -173.7(3) . .
F3 K2 F2 K5 65.60(19) . .
F3 K2 F2 K5 178.53(15) 8_557 .
F3 K2 F3 V1 -64.25(15) 8_557 .
F3 K2 F3 V2 127.31(19) 8_557 .
F3 K2 F3 K1 32.77(9) 8_557 9_557
F3 K2 F3 K5 -148.49(16) 8_557 .
F3 K2 F7 V3 36.2(3) . .
F3 K2 F7 V3 -179.5(3) 8_557 .
F3 K2 F7 K3 -72.99(16) . .
F3 K2 F7 K3 71.35(16) 8_557 .
F3 K2 F7 K4 -172.83(15) . 7_667
F3 K2 F7 K4 -28.49(19) 8_557 7_667
F3 K5 F2 V1 46.04(17) . .
F3 K5 F2 K2 -60.85(15) . .
F3 K5 F2 K3 -159.0(3) . .
F3 K5 F2D K5 127.0(14) . 2_665
F3 K5 F2D K5 -127.0(14) . 3_565
F3 K5 F5 V2 44.12(16) . .
F3 K5 F5 K2 -60.28(13) . 9_557
F3 K5 F5 K4 176.2(3) . 3_565
F3 K5 F8 V3 83.6(2) . 3_565
F3 K5 F8 K3 -29.68(18) . 9_556
F3 K5 F8 K4 -150.12(17) . 3_564
F3 K5 O3 V3 98.5(2) . .
F3 K5 O3 K4 -56.27(18) . .
F3 K5 O3 K5 -161.45(14) . 2_665
F4 V2 F3 V1 134.2(14) 10_556 .
F4 V2 F3 V1 -134.2(14) 1_556 .
F4 V2 F3 K1 45.81(14) 1_556 9_557
F4 V2 F3 K1 -45.81(14) 10_556 9_557
F4 V2 F3 K2 -133.19(18) 10_556 .
F4 V2 F3 K2 -41.57(16) 1_556 .
F4 V2 F3 K2 133.19(18) 1_556 9_557
F4 V2 F3 K2 41.57(16) 10_556 9_557
F4 V2 F3 K5 134.19(14) 10_556 .
F4 V2 F3 K5 -134.19(14) 1_556 .
F4 V2 F5 K2 -30.12(18) 10_556 9_557
F4 V2 F5 K2 54.9(8) 1_556 9_557
F4 V2 F5 K4 84.7(2) 10_556 3_565
F4 V2 F5 K4 169.7(6) 1_556 3_565
F4 V2 F5 K5 -139.1(2) 10_556 .
F4 V2 F5 K5 -54.0(8) 1_556 .
F4 V2 O2 K4 79.1(3) 1_556 .
F4 V2 O2 K4 -170.7(2) 1_556 3_565
F4 V2 O2 K4 170.7(2) 10_556 .
F4 V2 O2 K4 -79.1(3) 10_556 3_565
F4 V2 O2 K5 45.8(9) 10_556 1_556
F4 V2 O2 K5 -45.8(9) 1_556 1_556
F4 K1 F1 V1 100.4(4) 8_556 .
F4 K1 F1 V1 95.6(4) 6_556 .
F4 K1 F1 K1 -128.83(17) 8_556 9_557
F4 K1 F1 K1 -133.59(19) 6_556 9_557
F4 K1 F1 K2 -41.04(13) 6_556 .
F4 K1 F1 K2 -36.3(3) 8_556 .
F4 K2 F1 V1 81.6(2) 1_556 .
F4 K2 F1 V1 -111.8(3) 6_556 .
F4 K2 F1 K1 -18.54(12) 1_556 9_557
F4 K2 F1 K1 147.97(15) 6_556 9_557
F4 K2 F1 K1 -124.09(18) 1_556 .
F4 K2 F1 K1 42.42(15) 6_556 .
F4 K2 F2 V1 -55.9(2) 1_556 .
F4 K2 F2 V1 95.3(2) 6_556 .
F4 K2 F2 K3 -33.88(14) 6_556 .
F4 K2 F2 K3 174.97(15) 1_556 .
F4 K2 F2 K5 -154.60(19) 6_556 .
F4 K2 F2 K5 54.24(17) 1_556 .
F4 K2 F3 V1 -158.0(3) 1_556 .
F4 K2 F3 V1 -6.5(2) 6_556 .
F4 K2 F3 V2 -174.93(15) 6_556 .
F4 K2 F3 V2 33.56(16) 1_556 .
F4 K2 F3 K1 -60.97(16) 1_556 9_557
F4 K2 F3 K1 90.54(17) 6_556 9_557
F4 K2 F3 K5 117.8(2) 1_556 .
F4 K2 F3 K5 -90.73(16) 6_556 .
F4 K2 F7 V3 -18.3(3) 1_556 .
F4 K2 F7 V3 146.6(3) 6_556 .
F4 K2 F7 K3 37.38(12) 6_556 .
F4 K2 F7 K3 -127.47(12) 1_556 .
F4 K2 F7 K4 132.69(15) 1_556 7_667
F4 K2 F7 K4 -62.46(14) 6_556 7_667
F4 K3 F2 V1 -67.8(3) 6_556 .
F4 K3 F2 V1 64.4(3) . .
F4 K3 F2 K2 34.83(14) 6_556 .
F4 K3 F2 K2 167.07(17) . .
F4 K3 F2 K5 -84.1(2) . .
F4 K3 F2 K5 143.6(2) 6_556 .
F4 K3 F4 V2 140.6(3) 6_556 1_554
F4 K3 F4 K1 -13.22(12) 6_556 9_556
F4 K3 F4 K2 -106.03(12) 6_556 1_554
F4 K3 F6 V3 98.78(10) . .
F4 K3 F6 V3 -81.22(10) 6_556 .
F4 K3 F6 V3 -81.22(10) . 7_666
F4 K3 F6 V3 98.78(10) 6_556 7_666
F4 K3 F6 K4 -171.81(10) . 7_667
F4 K3 F6 K4 8.19(10) 6_556 7_667
F4 K3 F6 K4 8.19(10) . 1_554
F4 K3 F6 K4 -171.81(10) 6_556 1_554
F4 K3 F7 V3 179.38(18) 6_556 .
F4 K3 F7 V3 -45.5(3) . .
F4 K3 F7 K2 -39.56(14) 6_556 .
F4 K3 F7 K2 95.54(19) . .
F4 K3 F7 K4 75.32(13) 6_556 7_667
F4 K3 F7 K4 -149.58(18) . 7_667
F5 V2 F3 V1 -44.8(14) 10 .
F5 V2 F3 V1 44.9(14) . .
F5 V2 F3 K1 135.17(14) 10 9_557
F5 V2 F3 K1 -135.17(14) . 9_557
F5 V2 F3 K2 47.78(17) 10 .
F5 V2 F3 K2 -47.79(18) . 9_557
F5 V2 F3 K2 -137.45(18) 10 9_557
F5 V2 F3 K2 137.45(18) . .
F5 V2 F3 K5 44.83(14) . .
F5 V2 F3 K5 -44.83(14) 10 .
F5 V2 F5 K2 134.47(11) 10 9_557
F5 V2 F5 K4 -110.73(18) 10 3_565
F5 V2 F5 K5 25.5(3) 10 .
F5 V2 O2 K4 -99.9(2) . .
F5 V2 O2 K4 -10.2(3) 10 .
F5 V2 O2 K4 99.9(2) 10 3_565
F5 V2 O2 K4 10.2(3) . 3_565
F5 V2 O2 K5 -135.2(9) 10 1_556
F5 V2 O2 K5 135.2(9) . 1_556
F5 K2 F1 V1 -128.8(2) 8_557 .
F5 K2 F1 V1 30.9(2) 10 .
F5 K2 F1 K1 -174.84(16) 10 .
F5 K2 F1 K1 25.5(2) 8_557 .
F5 K2 F1 K1 -69.30(13) 10 9_557
F5 K2 F1 K1 131.01(13) 8_557 9_557
F5 K2 F2 V1 -99.2(2) 10 .
F5 K2 F2 V1 126.19(19) 8_557 .
F5 K2 F2 K3 -2.9(2) 8_557 .
F5 K2 F2 K3 131.69(17) 10 .
F5 K2 F2 K5 -123.67(15) 8_557 .
F5 K2 F2 K5 10.97(13) 10 .
F5 K2 F3 V1 1.2(7) 8_557 .
F5 K2 F3 V1 132.7(2) 10 .
F5 K2 F3 V2 -167.3(5) 8_557 .
F5 K2 F3 V2 -35.76(16) 10 .
F5 K2 F3 K1 -130.3(2) 10 9_557
F5 K2 F3 K1 98.2(6) 8_557 9_557
F5 K2 F3 K5 -83.1(6) 8_557 .
F5 K2 F3 K5 48.44(14) 10 .
F5 K2 F7 V3 -158.7(3) 8_557 .
F5 K2 F7 V3 -5.1(3) 10 .
F5 K2 F7 K3 92.16(13) 8_557 .
F5 K2 F7 K3 -114.33(13) 10 .
F5 K2 F7 K4 145.84(15) 10 7_667
F5 K2 F7 K4 -7.68(13) 8_557 7_667
F5 K4 O2 V2 9.1(2) 10 .
F5 K4 O2 V2 87.0(5) 2_665 .
F5 K4 O2 K4 -14.3(5) 2_665 3_565
F5 K4 O2 K4 -92.1(3) 10 3_565
F5 K4 O2 K5 166.2(3) 10 1_556
F5 K4 O2 K5 -116.0(3) 2_665 1_556
F5 K4 O3 V3 -100.09(13) 10 .
F5 K4 O3 V3 100.09(13) 2_665 .
F5 K4 O3 K5 -29.25(13) 2_665 2_665
F5 K4 O3 K5 130.6(2) 10 2_665
F5 K4 O3 K5 29.25(13) 10 .
F5 K4 O3 K5 -130.6(2) 2_665 .
F5 K5 F1D K5 86.8(7) . 2_665
F5 K5 F1D K5 -18.8(17) . 3_565
F5 K5 F1D K5 18.8(17) 10 2_665
F5 K5 F1D K5 -86.8(7) 10 3_565
F5 K5 F2 V1 46.2(2) . .
F5 K5 F2 V1 95.5(2) 10 .
F5 K5 F2 K2 -11.39(13) 10 .
F5 K5 F2 K2 -60.67(16) . .
F5 K5 F2 K3 -109.5(2) 10 .
F5 K5 F2 K3 -158.8(2) . .
F5 K5 F2D K5 99.2(13) 10 2_665
F5 K5 F2D K5 154.7(15) . 2_665
F5 K5 F2D K5 -99.2(13) . 3_565
F5 K5 F2D K5 -154.7(15) 10 3_565
F5 K5 F3 V1 143.25(13) . .
F5 K5 F3 V1 -143.25(13) 10 .
F5 K5 F3 V2 -36.75(13) . .
F5 K5 F3 V2 36.75(13) 10 .
F5 K5 F3 K2 53.59(14) . 9_557
F5 K5 F3 K2 -53.59(14) 10 .
F5 K5 F3 K2 -127.08(19) . .
F5 K5 F3 K2 127.08(19) 10 9_557
F5 K5 F5 V2 -20.2(2) 10 .
F5 K5 F5 K2 -124.64(9) 10 9_557
F5 K5 F5 K4 111.88(15) 10 3_565
F5 K5 F8 V3 34.6(2) . 3_565
F5 K5 F8 V3 44.7(4) 10 3_565
F5 K5 F8 K3 -68.6(3) 10 9_556
F5 K5 F8 K3 -78.70(17) . 9_556
F5 K5 F8 K4 160.87(18) . 3_564
F5 K5 F8 K4 171.0(2) 10 3_564
F5 K5 O3 V3 124.7(3) 10 .
F5 K5 O3 V3 149.3(2) . .
F5 K5 O3 K4 -5.4(2) . .
F5 K5 O3 K4 -29.99(15) 10 .
F5 K5 O3 K5 -110.60(16) . 2_665
F5 K5 O3 K5 -135.2(2) 10 2_665
F6 V3 K3 V3 0.0 . 7_666
F6 V3 K3 K2 -45.56(5) . 1_554
F6 V3 K3 F2 -168.30(13) . .
F6 V3 K3 F2 20.4(2) . 6_556
F6 V3 K3 F4 111.95(11) . 6_556
F6 V3 K3 F4 -98.55(11) . .
F6 V3 K3 F7 -27.42(9) . 6_556
F6 V3 K3 F7 112.57(18) . .
F6 V3 K3 F8 -111.78(16) . 10
F6 V3 K3 F8 28.08(8) . 8_556
F6 V3 F7 K2 -155.2(3) . .
F6 V3 F7 K3 -49.75(11) . .
F6 V3 F7 K4 51.65(10) . 7_667
F6 K3 F2 V1 177.2(3) . .
F6 K3 F2 K2 -80.12(12) . .
F6 K3 F2 K5 28.7(2) . .
F6 K3 F4 V2 -39.4(3) . 1_554
F6 K3 F4 K1 166.77(12) . 9_556
F6 K3 F4 K2 73.97(12) . 1_554
F6 K3 F7 V3 41.66(11) . .
F6 K3 F7 K2 -177.27(16) . .
F6 K3 F7 K4 -62.40(8) . 7_667
F6 K4 O2 V2 -102.4(3) 1_556 .
F6 K4 O2 K4 156.34(18) 1_556 3_565
F6 K4 O2 K5 54.7(2) 1_556 1_556
F6 K4 O3 V3 0.000(5) 1_556 .
F6 K4 O3 K5 -129.34(13) 1_556 2_665
F6 K4 O3 K5 129.34(13) 1_556 .
F7 V3 K3 V3 -112.57(18) . 7_666
F7 V3 K3 V3 -52.99(13) 12_665 7_666
F7 V3 K3 K2 -98.55(14) 12_665 1_554
F7 V3 K3 K2 -158.13(18) . 1_554
F7 V3 K3 F2 138.71(19) 12_665 .
F7 V3 K3 F2 79.1(2) . .
F7 V3 K3 F2 -92.2(3) . 6_556
F7 V3 K3 F2 -32.6(3) 12_665 6_556
F7 V3 K3 F4 58.96(17) 12_665 6_556
F7 V3 K3 F4 -151.54(16) 12_665 .
F7 V3 K3 F4 148.9(2) . .
F7 V3 K3 F4 -0.62(19) . 6_556
F7 V3 K3 F6 -52.99(13) 12_665 .
F7 V3 K3 F6 -112.57(18) . .
F7 V3 K3 F7 -139.99(14) . 6_556
F7 V3 K3 F7 -80.41(17) 12_665 6_556
F7 V3 K3 F7 59.6(2) 12_665 .
F7 V3 K3 F8 -164.8(2) 12_665 10
F7 V3 K3 F8 -84.49(19) . 8_556
F7 V3 K3 F8 135.6(2) . 10
F7 V3 K3 F8 -24.91(16) 12_665 8_556
F7 V3 F6 K3 -44.53(12) 12_665 7_666
F7 V3 F6 K3 135.47(12) 12_665 .
F7 V3 F6 K3 44.53(12) . .
F7 V3 F6 K3 -135.47(12) . 7_666
F7 V3 F6 K4 134.53(12) . 1_554
F7 V3 F6 K4 -134.53(12) 12_665 1_554
F7 V3 F6 K4 -45.47(12) . 7_667
F7 V3 F6 K4 45.47(12) 12_665 7_667
F7 V3 F7 K2 123.1(2) 12_665 .
F7 V3 F7 K3 -131.45(10) 12_665 .
F7 V3 F7 K4 -30.1(2) 12_665 7_667
F7 V3 O3 K4 45.51(13) . .
F7 V3 O3 K4 -45.51(13) 12_665 .
F7 V3 O3 K5 -84.8(2) . .
F7 V3 O3 K5 175.80(16) . 2_665
F7 V3 O3 K5 84.8(2) 12_665 2_665
F7 V3 O3 K5 -175.80(16) 12_665 .
F7 K2 F1 V1 74.8(5) 6_557 .
F7 K2 F1 V1 -52.2(3) . .
F7 K2 F1 K1 102.12(18) . .
F7 K2 F1 K1 -130.9(4) 6_557 .
F7 K2 F1 K1 -152.34(12) . 9_557
F7 K2 F1 K1 -25.4(5) 6_557 9_557
F7 K2 F2 V1 -134.6(2) 6_557 .
F7 K2 F2 V1 174.6(2) . .
F7 K2 F2 K3 45.46(14) . .
F7 K2 F2 K3 96.27(17) 6_557 .
F7 K2 F2 K5 -24.5(2) 6_557 .
F7 K2 F2 K5 -75.26(15) . .
F7 K2 F3 V1 157.92(15) 6_557 .
F7 K2 F3 V1 75.12(19) . .
F7 K2 F3 V2 -10.5(2) 6_557 .
F7 K2 F3 V2 -93.32(18) . .
F7 K2 F3 K1 -105.05(15) 6_557 9_557
F7 K2 F3 K1 172.15(13) . 9_557
F7 K2 F3 K5 -9.12(17) . .
F7 K2 F3 K5 73.68(16) 6_557 .
F7 K2 F7 V3 -74.4(3) 6_557 .
F7 K2 F7 K3 176.5(2) 6_557 .
F7 K2 F7 K4 76.63(14) 6_557 7_667
F7 K3 F2 V1 118.8(3) 6_556 .
F7 K3 F2 V1 -145.1(3) . .
F7 K3 F2 K2 -42.42(12) . .
F7 K3 F2 K2 -138.57(15) 6_556 .
F7 K3 F2 K5 66.4(2) . .
F7 K3 F2 K5 -29.8(3) 6_556 .
F7 K3 F4 V2 22.7(4) . 1_554
F7 K3 F4 V2 -75.9(3) 6_556 1_554
F7 K3 F4 K1 130.24(19) 6_556 9_556
F7 K3 F4 K1 -131.13(19) . 9_556
F7 K3 F4 K2 37.43(13) 6_556 1_554
F7 K3 F4 K2 136.06(15) . 1_554
F7 K3 F6 V3 -34.92(12) . .
F7 K3 F6 V3 145.08(12) . 7_666
F7 K3 F6 V3 -34.92(12) 6_556 7_666
F7 K3 F6 V3 145.08(12) 6_556 .
F7 K3 F6 K4 54.49(11) 6_556 1_554
F7 K3 F6 K4 54.49(11) . 7_667
F7 K3 F6 K4 -125.51(11) . 1_554
F7 K3 F6 K4 -125.51(11) 6_556 7_667
F7 K3 F7 V3 41.66(11) 6_556 .
F7 K3 F7 K2 -177.27(16) 6_556 .
F7 K3 F7 K4 -62.40(8) 6_556 7_667
F7 K4 O2 V2 -65.3(5) 7_667 .
F7 K4 O2 V2 -51.5(3) 6_557 .
F7 K4 O2 K4 -166.61(15) 7_667 3_565
F7 K4 O2 K4 -152.8(2) 6_557 3_565
F7 K4 O2 K5 105.5(2) 6_557 1_556
F7 K4 O2 K5 91.7(3) 7_667 1_556
F7 K4 O3 V3 27.6(3) 7_667 .
F7 K4 O3 V3 -27.6(3) 6_557 .
F7 K4 O3 K5 -101.71(14) 7_667 2_665
F7 K4 O3 K5 156.97(16) 7_667 .
F7 K4 O3 K5 -156.97(16) 6_557 2_665
F7 K4 O3 K5 101.71(14) 6_557 .
F8 V3 K3 V3 111.78(16) 10 7_666
F8 V3 K3 V3 54.85(15) 2_665 7_666
F8 V3 K3 K2 9.29(16) 2_665 1_554
F8 V3 K3 K2 66.22(16) 10 1_554
F8 V3 K3 F2 -56.5(2) 10 .
F8 V3 K3 F2 -113.4(2) 2_665 .
F8 V3 K3 F2 132.1(3) 10 6_556
F8 V3 K3 F2 75.2(3) 2_665 6_556
F8 V3 K3 F4 -136.27(19) 10 6_556
F8 V3 K3 F4 166.80(18) 2_665 6_556
F8 V3 K3 F4 13.24(19) 10 .
F8 V3 K3 F4 -43.69(19) 2_665 .
F8 V3 K3 F6 54.85(15) 2_665 .
F8 V3 K3 F6 111.78(16) 10 .
F8 V3 K3 F7 -135.6(2) 10 .
F8 V3 K3 F7 167.4(2) 2_665 .
F8 V3 K3 F7 84.37(18) 10 6_556
F8 V3 K3 F7 27.43(17) 2_665 6_556
F8 V3 K3 F8 82.94(18) 2_665 8_556
F8 V3 K3 F8 139.87(14) 10 8_556
F8 V3 K3 F8 -56.9(2) 2_665 10
F8 V3 F6 K3 46.19(13) 2_665 7_666
F8 V3 F6 K3 -133.81(13) 2_665 .
F8 V3 F6 K3 133.81(13) 10 7_666
F8 V3 F6 K3 -46.19(13) 10 .
F8 V3 F6 K4 136.19(13) 2_665 7_667
F8 V3 F6 K4 43.81(13) 10 1_554
F8 V3 F6 K4 -43.81(13) 2_665 1_554
F8 V3 F6 K4 -136.19(13) 10 7_667
F8 V3 F7 K2 -149.2(6) 2_665 .
F8 V3 F7 K2 -72.9(3) 10 .
F8 V3 F7 K3 -43.8(7) 2_665 .
F8 V3 F7 K3 32.58(17) 10 .
F8 V3 F7 K4 57.6(7) 2_665 7_667
F8 V3 F7 K4 133.98(16) 10 7_667
F8 V3 O3 K4 136.23(13) 10 .
F8 V3 O3 K4 -136.23(13) 2_665 .
F8 V3 O3 K5 -93.48(17) 10 2_665
F8 V3 O3 K5 -5.9(2) 2_665 2_665
F8 V3 O3 K5 5.9(2) 10 .
F8 V3 O3 K5 93.48(17) 2_665 .
F8 K3 F2 V1 -134.9(3) 8_556 .
F8 K3 F2 V1 156.1(4) 10 .
F8 K3 F2 K2 -101.21(16) 10 .
F8 K3 F2 K2 -32.2(4) 8_556 .
F8 K3 F2 K5 7.60(17) 10 .
F8 K3 F2 K5 76.6(4) 8_556 .
F8 K3 F4 V2 6.3(3) 10 1_554
F8 K3 F4 V2 -101.0(3) 8_556 1_554
F8 K3 F4 K1 105.15(19) 8_556 9_556
F8 K3 F4 K1 -147.55(18) 10 9_556
F8 K3 F4 K2 12.3(2) 8_556 1_554
F8 K3 F4 K2 119.64(13) 10 1_554
F8 K3 F6 V3 35.73(10) 8_556 7_666
F8 K3 F6 V3 -144.27(10) 10 7_666
F8 K3 F6 V3 -144.27(10) 8_556 .
F8 K3 F6 V3 35.73(10) 10 .
F8 K3 F6 K4 125.14(10) 10 7_667
F8 K3 F6 K4 -54.86(10) 10 1_554
F8 K3 F6 K4 125.14(10) 8_556 1_554
F8 K3 F6 K4 -54.86(10) 8_556 7_667
F8 K3 F7 V3 -25.42(14) 10 .
F8 K3 F7 V3 91.46(17) 8_556 .
F8 K3 F7 K2 -127.47(13) 8_556 .
F8 K3 F7 K2 115.65(16) 10 .
F8 K3 F7 K4 -12.60(11) 8_556 7_667
F8 K3 F7 K4 -129.48(15) 10 7_667
F8 K4 O2 V2 -128.8(4) 10_556 .
F8 K4 O2 V2 -155.7(3) 2_666 .
F8 K4 O2 K4 103.1(2) 2_666 3_565
F8 K4 O2 K4 129.9(3) 10_556 3_565
F8 K4 O2 K5 1.4(2) 2_666 1_556
F8 K4 O2 K5 28.25(15) 10_556 1_556
F8 K4 O3 V3 -70.5(3) 10_556 .
F8 K4 O3 V3 70.5(3) 2_666 .
F8 K4 O3 K5 -160.2(3) 2_666 .
F8 K4 O3 K5 160.2(3) 10_556 2_665
F8 K4 O3 K5 58.9(4) 10_556 .
F8 K4 O3 K5 -58.9(4) 2_666 2_665
F8 K5 F1D K5 -170.9(15) 10 3_565
F8 K5 F1D K5 170.9(15) . 2_665
F8 K5 F1D K5 -65.2(10) 10 2_665
F8 K5 F1D K5 65.2(10) . 3_565
F8 K5 F2 V1 -50.1(2) . .
F8 K5 F2 V1 -163.0(3) 10 .
F8 K5 F2 K2 -156.96(14) . .
F8 K5 F2 K2 90.15(17) 10 .
F8 K5 F2 K3 -7.97(17) 10 .
F8 K5 F2 K3 104.9(2) . .
F8 K5 F2D K5 8.5(17) 10 2_665
F8 K5 F2D K5 -114.5(11) . 2_665
F8 K5 F2D K5 -8.5(17) . 3_565
F8 K5 F2D K5 114.5(11) 10 3_565
F8 K5 F3 V1 63.39(10) . .
F8 K5 F3 V1 -63.39(10) 10 .
F8 K5 F3 V2 -116.61(10) . .
F8 K5 F3 V2 116.61(10) 10 .
F8 K5 F3 K2 26.27(17) 10 .
F8 K5 F3 K2 153.05(13) . .
F8 K5 F3 K2 -26.28(17) . 9_557
F8 K5 F3 K2 -153.05(13) 10 9_557
F8 K5 F5 V2 -7.8(4) 10 .
F8 K5 F5 V2 153.0(2) . .
F8 K5 F5 K2 -112.2(3) 10 9_557
F8 K5 F5 K2 48.58(16) . 9_557
F8 K5 F5 K4 -74.9(2) . 3_565
F8 K5 F5 K4 124.3(3) 10 3_565
F8 K5 F8 V3 -157.24(11) 10 3_565
F8 K5 F8 K3 89.5(2) 10 9_556
F8 K5 F8 K4 -30.9(3) 10 3_564
F8 K5 O3 V3 -77.3(4) . .
F8 K5 O3 V3 -5.20(18) 10 .
F8 K5 O3 K4 128.0(3) . .
F8 K5 O3 K4 -159.9(2) 10 .
F8 K5 O3 K5 94.9(2) 10 2_665
F8 K5 O3 K5 22.8(4) . 2_665
O1 V1 F1 K1 -4.7(5) . .
O1 V1 F1 K1 -136.9(3) . 9_557
O1 V1 F1 K2 129.8(3) . .
O1 V1 F2 K2 -127.0(3) . .
O1 V1 F2 K3 -30.3(4) . .
O1 V1 F2 K5 121.7(3) . .
O1 K1 F1 V1 35.6(5) 8_556 .
O1 K1 F1 K1 166.4(2) 8_556 9_557
O1 K1 F1 K2 -101.1(2) 8_556 .
O2 V2 F5 K2 -128.6(3) . 9_557
O2 V2 F5 K4 -13.8(3) . 3_565
O2 V2 F5 K5 122.5(3) . .
O2 K4 O2 V2 146.5(2) 2_665 .
O2 K4 O2 K4 45.2(4) 2_665 3_565
O2 K4 O2 K5 -56.5(4) 2_665 1_556
O2 K4 O3 V3 115.76(16) 2_665 .
O2 K4 O3 V3 -115.76(16) . .
O2 K4 O3 K5 13.6(2) . .
O2 K4 O3 K5 -114.9(2) 2_665 .
O2 K4 O3 K5 114.9(2) . 2_665
O2 K4 O3 K5 -13.6(2) 2_665 2_665
O2 K5 F1D K5 127.2(12) 1_554 3_565
O2 K5 F1D K5 -127.2(12) 1_554 2_665
O2 K5 F2 V1 -98.1(2) 1_554 .
O2 K5 F2 K2 155.06(18) 1_554 .
O2 K5 F2 K3 56.9(2) 1_554 .
O2 K5 F2D K5 53.0(14) 1_554 3_565
O2 K5 F2D K5 -53.0(14) 1_554 2_665
O2 K5 F3 V1 0.0 1_554 .
O2 K5 F3 V2 180.0 1_554 .
O2 K5 F3 K2 -89.67(11) 1_554 9_557
O2 K5 F3 K2 89.66(11) 1_554 .
O2 K5 F5 V2 115.6(3) 1_554 .
O2 K5 F5 K2 11.2(4) 1_554 9_557
O2 K5 F5 K4 -112.3(3) 1_554 3_565
O2 K5 F8 V3 -169.6(3) 1_554 3_565
O2 K5 F8 K3 77.1(3) 1_554 9_556
O2 K5 F8 K4 -43.3(3) 1_554 3_564
O2 K5 O3 V3 -19.0(3) 1_554 .
O2 K5 O3 K4 -173.7(2) 1_554 .
O2 K5 O3 K5 81.1(2) 1_554 2_665
O3 V3 K3 V3 179.5(3) . 7_666
O3 V3 K3 K2 133.9(3) . 1_554
O3 V3 K3 F2 11.2(3) . .
O3 V3 K3 F2 -160.1(4) . 6_556
O3 V3 K3 F4 81.0(3) . .
O3 V3 K3 F4 -68.5(3) . 6_556
O3 V3 K3 F6 179.5(3) . .
O3 V3 K3 F7 -67.9(4) . .
O3 V3 K3 F7 152.1(3) . 6_556
O3 V3 K3 F8 67.7(4) . 10
O3 V3 K3 F8 -152.4(3) . 8_556
O3 V3 F7 K2 24.5(3) . .
O3 V3 F7 K3 130.0(2) . .
O3 V3 F7 K4 -128.6(2) . 7_667
O3 K4 O2 V2 27.4(4) . .
O3 K4 O2 K4 -73.9(3) . 3_565
O3 K4 O2 K5 -175.6(2) . 1_556
O3 K5 F1D K5 13.5(10) 3_565 3_565
O3 K5 F1D K5 119.1(15) 3_565 2_665
O3 K5 F1D K5 -13.5(10) . 2_665
O3 K5 F1D K5 -119.1(15) . 3_565
O3 K5 F2 V1 -0.5(4) 3_565 .
O3 K5 F2 V1 150.9(2) . .
O3 K5 F2 K2 -107.4(2) 3_565 .
O3 K5 F2 K2 43.98(17) . .
O3 K5 F2 K3 154.5(2) 3_565 .
O3 K5 F2 K3 -54.1(2) . .
O3 K5 F2D K5 -42.5(7) 3_565 3_565
O3 K5 F2D K5 149(2) . 3_565
O3 K5 F2D K5 -149(2) 3_565 2_665
O3 K5 F2D K5 42.5(7) . 2_665
O3 K5 F3 V1 -114.73(12) . .
O3 K5 F3 V1 114.73(12) 3_565 .
O3 K5 F3 V2 65.27(12) . .
O3 K5 F3 V2 -65.27(12) 3_565 .
O3 K5 F3 K2 155.60(15) . 9_557
O3 K5 F3 K2 -155.60(15) 3_565 .
O3 K5 F3 K2 -25.07(18) . .
O3 K5 F3 K2 25.07(18) 3_565 9_557
O3 K5 F5 V2 -45.2(2) . .
O3 K5 F5 V2 -170.7(3) 3_565 .
O3 K5 F5 K2 84.91(17) 3_565 9_557
O3 K5 F5 K2 -149.58(14) . 9_557
O3 K5 F5 K4 86.9(2) . 3_565
O3 K5 F5 K4 -38.57(18) 3_565 3_565
O3 K5 F8 V3 -4.81(17) 3_565 3_565
O3 K5 F8 V3 -100.8(4) . 3_565
O3 K5 F8 K3 -118.1(2) 3_565 9_556
O3 K5 F8 K3 146.0(3) . 9_556
O3 K5 F8 K4 25.5(4) . 3_564
O3 K5 F8 K4 121.5(2) 3_565 3_564
O3 K5 O3 V3 -152.71(14) 3_565 .
O3 K5 O3 K4 52.6(3) 3_565 .
O3 K5 O3 K5 -52.6(3) 3_565 2_665
